Home >
Documents >
POLITECNICO DI MILANO - Home | POLITesi · POLITECNICO DI MILANO Scuola di Ingegneria dei Processi...

Share this document with a friend

Embed Size (px)

of 132
/132

Transcript

POLITECNICO DI MILANO

Scuola di Ingegneria dei Processi Industriali

Dipartimento di Chimica, Materiali e Ingegneria Chimica “G. Natta”

Master of science in Materials engineering and Nanotechnologies

PROBABILITY OF STAINLESS STEEL

CORROSION: EXPERIMENTAL VALIDATION OF

THE MARKOV’S CHAINS MATHEMATICAL

MODEL

Tutor: Prof. Marco ORMELLESE

Co-tutor: Ing. Andrea BRENNA

Anno accademico 2012-2013

Chiara DE ANGELIS

Matr. 770400

CONTENTS

CONTENTS

CONTENTS OF FIGURES ................................................................................................. I

CONTENTS OF TABLES ................................................................................................ IV

CONTENTS OF PLOTS .................................................................................................. VI

ABSTRACT ......................................................................................................................... 1

INTRODUZIONE ............................................................................................................... 2

1. CORROSION OF STAINLESS STEEL: AN OVERVIEW ..................................... 4

1.1 STAINLESS STEELS .................................................................................................. 4

1.1.1 Austenitic stainless steels ...................................................................................... 5

1.1.2 Ferritic stainless steels ........................................................................................... 6

1.1.3 Martensitic stainless steels..................................................................................... 7

1.1.4 Duplex stainless steels ........................................................................................... 7

1.2 CORROSION FORMS OF STAINLESS STEEL ....................................................... 8

1.2.1 General corrosion .................................................................................................. 8

1.2.2 Localized corrosion ............................................................................................... 8

1.3 PITTING CORROSION............................................................................................... 9

1.3.1 Pitting corrosion mechanism ................................................................................. 9

1.3.2 Thermodynamic and kinetic aspects of pitting corrosion ...................................... 9

1.3.3 Effect of stainless steels composition on pitting resistance ................................. 14

1.3.4 Effect of microstructure on pitting behavior of stainless steel ............................ 18

1.3.5 Effect of surface finish on pitting behavior of stainless steel .............................. 18

1.3.6 Effect of environmental parameters on pitting resistance of stainless steel ........ 19

1.4 CREVICE CORROSION ........................................................................................... 21

2. MARKOV MODEL: STATE OF ART ..................................................................... 24

2.1 INTRODUCTION ............................................................................................................... 24

2.2 MARKOV CHAINS .................................................................................................. 25

2.3 THREE STEPS MARKOV MODEL ............................................................................... 30

2.4 FIVE STEPS MARKOV MODEL .................................................................................... 31

2.4.1 Transitional probabilities relation with input parameters .................................... 33

2.4.2 Transitional probability m: meta-stable to meta-passive transition…………… 34

2.4.3 Transitional probability r: meta-passive to passive transition ............................. 38

CONTENTS

2.4.4 Transitional probability p: meta-pitting to pitting transition ................................ 40

2.4.5 Example of R calculation ..................................................................................... 41

2.5 STATISTICAL EVALUATION OF CORROSION DATA .......................................... 44

2.5.1 Corrosion data distributions................................................................................. 45

2.5.2 Extreme value statistics ....................................................................................... 48

3. VALIDATION OF THE PROPOSED MARKOV MODEL: POTENTIOSTATIC

POLARIZATION TEST ................................................................................................... 53

3.1 AIM OF THE TEST ............................................................................................................ 53

3.2 POTENTIOSTATIC POLARIZATION TEST ............................................................... 53

3.3 EXPERIMENTAL SET UP ............................................................................................... 54

3.3.1 Samples preparation ............................................................................................. 54

3.3.2 Electrochemical cells assembly ............................................................................ 56

3.3.3 Experimental procedure ....................................................................................... 58

3.4 RESULTS AND DISCUSSION ......................................................................................... 61

4. p-PROBABILITY: A REVIEW OF THE META-PITTING TO PITTING

TRANSITION .................................................................................................... …………68

4.1 INTRODUCTION ....................................................................................................... 68

4.2 STATISTICAL ELABORATION OF LITERATURE DATA .................................. 70

4.2.1 Pitting potential distribution ................................................................................ 70

4.2.2 Protection potential determination ...................................................................... 72

4.2.3 Calculation of p-probability ................................................................................ 74

4.3 CYCLIC POTENTIODYNAMIC POLARIZATION TESTS ................................... 76

4.3.1 Experimental set up ............................................................................................. 78

4.3.2 Results and discussion ......................................................................................... 79

4.3.2.1 AISI 430 stainless steel................................................................................ 79

4.3.2.2 AISI 304 stainless steel................................................................................ 81

4.3.2.3 AISI 470LI stainless steel ............................................................................ 83

4.3.2.4 Protection potential-PREN curve: experimental and theoretical values

comparison. ................................................................................................................. 85

4.4 p-PROBABILITY CURVE: EXPERIMENTAL AND THEORETICAL VALUES

COMPARISON ................................................................................................................... 85

CONTENTS

5. m-PROBABILITY: A REVIEW OF THE META-STABLE TO META-PASSIVE

TRANSITION .................................................................................................................... 88

5.1 INTRODUCTION ...................................................................................................... 88

5.2 LINEAR POLARIZATION RESISTANCE TEST ................................................... 90

5.3 EFFECT OF pH ON CRITICAL CHLORIDES THRESHOLD ............................... 93

5.3.1 Aim of the test ..................................................................................................... 93

5.3.2 Experimental set-up ............................................................................................. 93

5.3.3 Results ................................................................................................................. 96

5.3.3.1 pH= 2 ............................................................................................................ 96

5.3.3.2 pH= 7 ............................................................................................................ 98

5.3.3.3 pH= 12 ........................................................................................................ 100

5.3.4 Discussion .......................................................................................................... 101

5.4 EFFECT OF TEMPERATURE ON CRITICAL CHLORIDES THRESHOLD ..... 103

5.4.1 Aim of the test ................................................................................................... 103

5.4.2 Experimental set up ........................................................................................... 103

5.4.3 Results ............................................................................................................... 104

5.4.4 Discussion .......................................................................................................... 101

5.5 CALCULATION OF m-PROBABILITY ............................................................... 107

6. CONCLUSION .......................................................................................................... 110

6.1 p-probability: new Markov model equations. ...................................................... 111

6.2 m-probability: new Markov model equation. ....................................................... 111

6.2 r-probability: the existing Markov model equation. ............................................. 112

6.3 Final consideration and future perspective. .......................................................... 112

APPENDIX A: Literature data collection. ....................................................................... 115

APPENDIX B: Density and cumulative distribution of the collected pitting potential.... 117

REFERENCES.... ............................................................................................................ 119

CONTENTS OF FIGURES

I

CONTENTS OF FIGURES

Figure 1.1- Schaeffler diagram ............................................................................................. 5

Figure 1.2- Typical shape of pitting corrosion attack ........................................................... 9

Figure 1.3- Pitting corrosion attack mechanism ................................................................. 10

Figure 1.4- Chromium Pourbaix diagram ........................................................................... 11

Figure 1.5- Chromium Pourbaix diagram in solution containing chlorides ....................... 11

Figure 1.6- Evan’s diagram: anodic curve of a passive metal and cathodic curve (red line)

arising from oxidizing condition…………………………………………………………. 12

Figure 1.7- Anodic curve of stainless steel. ........................................................................ 13

Figure 1.8- Effect of chlorides of anodic curve of stainless steel. ...................................... 13

Figure 1.9- Anodic curve of a passive metal: Epitt and Eprot definition ............................... 14

Figure 1.10- Pedeferri diagram ........................................................................................... 14

Figure 1.11- Effect of some alloying elements on the anodic polarization curve of stainless

steel ...................................................................................................................................... 15

Figure 1.12- Effect of chromium content on pitting potential of iron-chromium alloys in

deareated 0.1 N NaCl solution at 25 °C .............................................................................. 16

Figure 1.13- Effect of molybdenum content on pitting potential of Fe-15% Cr-13% Ni

alloys in a deareated 0.1 N NaCl solution at 25°C .............................................................. 16

Figure 1.14- Effect of nickel content on pitting potential of Fe-15% Cr alloys in a

deareated 0.1 N NaCl solution at 25 °C .............................................................................. 17

Figure 1.15- Effect of PREN on pitting potential of stainless steel in a 0.6 M NaCl solution

at 25°C (21000 ppm Cl-). ..................................................................................................... 17

Figure 1.16- Effect of chloride ions on the polarization curve of stainless steel ............... 19

Figure 1.17- Effect of chlorides concentration on the pitting potential of AISI 316 and 304

at room temperature in a 3% NaCl solution ........................................................................ 19

Figure 1.18- Effect of temperature on the pitting potential of various stainless steels in a

3% NaCl solution. ............................................................................................................... 20

Figure 1.19-Effect of pH on pitting potential of various stainless steels in a 3% NaCl

solution ................................................................................................................................ 20

Figure 1.20- Crevice corrosion: (a) crevice resulting from the joining of the two plates of

steel; (b) crevice due to a gasket between two flanged pipes .............................................. 21

CONTENTS OF FIGURES

II

Figure 1.21- Schematic illustration of the crevice corrosion mechanism .......................... 22

Figure 2.1- Standard rating charts for pits .......................................................................... 25

Figure 2.2- Schematization of the three steps Markov model ............................................ 30

Figure 2.3- Schematization of the five steps Markov model .............................................. 31

Figure 2.4- Scheme of the influence factors of the transitional probabilities ..................... 34

Figure 2.5- k dependence of m-probability......................................................................... 35

Figure 2.6- Critical chlorides threshold dependence of pH ................................................ 37

Figure 2.7- Critical chlorides threshold dependence of temperature and effect of crevice

(dashed lines) ....................................................................................................................... 38

Figure 2.8- Velocity dependence of r probability .............................................................. 39

Figure 2.9- Potential dependence of p probability ............................................................. 40

Figure 2.10- PREN dependence of protection potential. .................................................... 41

Figure 2.11- Matlab implementation of the Markov model ............................................... 42

Figure 2.12- Demonstration of the concept of corrosion probability by Mears and Evans 45

Figure 2.13- Normal (Gaussian) distribution...................................................................... 46

Figure 2.14- Probability plot for the distribution of pitting potential on normal probability

paper .................................................................................................................................... 47

Figure 2.15- Distribution curves of pits obeying the Poisson distribution ......................... 48

Figure 2.16- Probability plot of the distribution of pit depth in samples of small area on

Gumbel probability paper, from which the maximum pit depth for the larger surface area

can be extimated .................................................................................................................. 50

Figure 2.17- Probability plots on Weibull probability paper of the SCC failure time of

austenitic stainless steel in boiling MgCl2 solution ............................................................. 51

Figure 2.18- Weibull probability plots of the SCC failure time of high strength steel bolts

exposed under various environmental conditions ............................................................... 51

Figure 3.1- Schematic representation of an experimental set up ........................................ 54

Figure 3.2- Stainless steel sample 3x3 cm. ......................................................................... 55

Figure 3.3- Welded cable on the sample back surface ....................................................... 55

Figure 3.4- Coated back surface ......................................................................................... 55

Figure 3.5- Exposed surface (2x2 cm). ............................................................................... 55

Figure 3.6- Scheme of the test cell and electrical connections. .......................................... 56

Figure 3.7- Cell cover with holes ....................................................................................... 57

CONTENTS OF FIGURES

III

Figure 3.8- Reference electrode, counter electrode and samples in the test cell. ............... 57

Figure 3.9- Electrical connection of the electrochemical cells to the potentiosta .............. 57

Figure 3.10- Ohmic drop on the resistance measurement .................................................. 58

Figure 4.1- Potential dependence of p probability ............................................................. 69

Figure 4.2- Effect of chromium content on pitting potential of iron-chromium alloys ...... 70

Figure 4.3- Cyclic polarization curve for a passive metal .................................................. 77

Figure 4.4- Electrochemical cell ......................................................................................... 79

Figure 5.1- k dependence of m-probability......................................................................... 88

Figure 5.2- Critical chlorides threshold dependence of pH: theoretical curves predicted by

Markov model for different stainless steel at 20°C and kcr= 0. ........................................... 89

Figure 5.3- Critical chlorides threshold dependence of temperature: theoretical curves

predicted by Markov model for different stainless steels at pH 7 and Kcr equal to zero ..... 90

Figure 5.4- Schematic representation of the electrochemical cell: CE is the counter

electrode (Ti-MMO), W the working electrode (stainless steel sample) and ER the

reference electrode (SSCsat). .............................................................................................. 91

Figure 5.5 Measurement of icorr by linear polarization ...................................................... 92

Figure 5.6- Schematic illustration of the electrochemical concept of potential decrease .. 93

Figure 5.7- Sample in the teflon couvette ........................................................................... 94

Figure 5.8- Finished sample ............................................................................................... 94

Figure 5.9- Cables passage into cover holes and sample immersion ................................. 95

Figure 5.10- Becker cover .................................................................................................. 95

Figure 5.11- Electrical connection and monitoring. ........................................................... 95

Figure 5.12- 40° C test set up and cables for potential and LPR monitoring. .................. 103

Figure 6.1- Five-step Markov model. ............................................................................... 110

CONTENTS OF TABLES

IV

CONTENTS OF TABLES

Table 1.1- General chemical composition of austenitic stainless steels available on the market ....... 6

Table 1.2- General chemical composition of ferritic stainless steels available on the market ............ 6

Table 1.3- General chemical composition of martensitic stainless steels available on the market ..... 7

Table 1.4- General chemical composition of duplex stainless steels available on the market ............ 8

Table 2.1- AISI 304, pH= 7, E= 0 V SCE ......................................................................................... 43

Table 2.2- AISI 304, E= 0 V SCE, v= 1,5 m/s, T=20 °C .................................................................. 43

Table 2.3- AISI 316, pH=7, E= 0,100 V SCE ................................................................................... 43

Table 2.4- AISI 316, E= 0,100 V SCE, v=1,5 m/s, T=20°C ............................................................. 44

Table 2.5- Examples of probability distribution in corrosion ........................................................... 45

Table 3.1- Chemical composition of the test materials ..................................................................... 53

Table 3.2- Experimental condition, 20°C, E1 .................................................................................... 59

Table 3.3- Experimental conditions 20°C, E2 ................................................................................... 60

Table 3.4- Experimental conditions 40°C, E1 ................................................................................... 60

Table 3.5- Experimental conditions 40°C, E2* ................................................................................. 60

Table 3.5- Results of potentiostatic test at E1 and E2 on AISI 430 at 25 and 40°C .......................... 61

Table 3.6- Results of potentiostatic test at E1 and E2 on AISI 304 at 25 and 40°C ......................... 61

Table 3.7- Results of potentiostatic test at E1 and E2 on 470LI stainless steel at 25 and 40°C......... 61

Table 3.8- AISI 430 (PREN 17) experimental corrosion probability and Markov probabilities ...... 63

Table 3.9- AISI 304 (PREN 18) experimental corrosion probability and Markov probabilities ...... 65

Table 3.10- 470 LI (PREN 24) experimental corrosion probability and Markov probabilities ........ 66

Table 4.2- Experimental values of pitting and protection potential .................................................. 81

Table 4.3- Mean experimental values and Markov model values for AISI 430 stainless steel ........ 81

Table 4.4- Experimental values of pitting and protection potential .................................................. 83

Table 4.5- Mean experimental values and Markov model values for AISI 304 stainless steel ........ 83

Table 4.6- Experimental values of pitting and protection potential ................................................. 84

Table 5.1- Critical chlorides threshold at pH 2. ................................................................................ 96

Table 5.2- Critical chlorides threshold at pH 7 ................................................................................. 98

Table 5.3- Critical chlorides threshold at 40°C ............................................................................... 104

Table 5.5- pH dependence of old Markov and new Markov model m-probability ......................... 107

Table 5.6- Temperature dependence of old Markov and new Markov model m-probability ......... 108

Table 5.7- Chlorides concentration dependence of old and new Markov model m-probability ..... 108

Table 6.1- AISI 430 (PREN 17) experimental corrosion probability and Markov probabilities .... 113

CONTENTS OF TABLES

V

Table 6.2- AISI 304 (PREN 18) experimental corrosion probability and Markov probabilities. ... 113

Table 6.3- 470LI (PREN 24) experimental corrosion probability and Markov probabilities ......... 114

CONTENTS OF PLOTS

VI

CONTENTS OF PLOTS

Plot 3.1- Experimental and theoretical corrosion probability comparison for AISI 430 at 20°C. .... 64

Plot 3.2- Experimental and theoretical corrosion probability comparison for AISI 430 at 40°C. .... 64

Plot 3.3- Experimental and theoretical corrosion probability comparison for AISI 304 at 20°C ..... 65

Plot 3.4- Experimental and theoretical corrosion probability comparison for AISI 304 at 40°C ..... 66

Plot 3.5- Experimental and theoretical corrosion probability comparison for 470 LI at 20°C ......... 67

Plot 3.6- Experimental and theoretical corrosion probability comparison for 470 LI at 40°C. ........ 67

Plot 4.1- Selected data are reported on a potential-PREN graph, compared with curve of Fig. 4.2

and values scattering is underlined .................................................................................................... 71

Plot 4.2- Cumulative probability function curve and definition of pitting potential ......................... 72

Plot 4.3- Normal distribution function curve of pitting potential ...................................................... 72

Plot 4.4- Protection potential determination ...................................................................................... 73

Plot 4.5- Eprot-PREN trend. ................................................................................................................ 74

Plot 4.6- p probability- (E- Eprot) trend .............................................................................................. 75

Plot 4.7- p probability-potential trend for different stainless steels: comparison between new and

old Markov model. ............................................................................................................................. 76

Plot 4.8- Cyclic potentio8ynamic curve for AISI 430 (PREN 17) in 20 g/L NaCl solution ............. 80

Plot 4.9- Potentiodynamic curve for AISI 304 in 20 g/L NaCl solution ........................................... 82

Plot 4.10- Potentiodynamic curve for AISI 470LI in 20 g/L NaCl solution ..................................... 84

Plot 4.11- Eprot-PREN trend: theoretical and experimental comparison ............................................ 85

Plot 4.12- p-probability curve for AISI 430 stainless steel and experimental values ....................... 86

Plot 4.13- p-probability curve for AISI 304 stainless steel and experimental values ....................... 87

Plot 5.1- Potential- time trend at pH 2 ............................................................................................... 97

Plot 5.2- LPR-time trend at pH 2 ....................................................................................................... 97

Plot 5.3- Potential-time trend at pH 7 ................................................................................................ 99

Plot 5.4- LPR-time trend at pH 7 ....................................................................................................... 99

Plot 5.5- Potential-time trend at pH 12 ............................................................................................ 100

Plot 5.6- LPR-time trend at pH 12 ................................................................................................... 100

Plot 5.7- Experimental data elaboration: reviewed pH-chlorides threshold trend .......................... 102

Plot 5.8- Potential-time trend at 40°C ............................................................................................. 104

Plot 5.9- LPR-time trend at 40°C .................................................................................................... 104

Plot 5.10- Experimental data elaboration: reviewed temperature-chlorides threshold trend .......... 106

ABSTRACT

1

ABSTRACT

Stainless steels are widely used in industrial application for their corrosion resistance;

nevertheless, in presence of chloride ions, they may be subject of localized corrosion

attack, as pitting and crevice, which, once initiated, rapidly propagates and leads to

equipment failure. Due to the stochastic nature of pitting phenomenon and, in particular, of

its initiation, a statistical approach is mandatory for initiation time prediction and, then, for

materials selection in engineering application. In this work is proposed a Markov chain’s

mathematical model which assumes that pitting retains no memory of its past history and is

characterized by two absorbing conditions (pitting and repassivation) and three transitional

states (metastable, metapassive, metapitting); the model takes into account metallurgical

and environmental factors, as material composition (PREN), chlorides concentration, pH,

temperature, fluidodynamic condition and oxidant power of the system, with the aim to

calculate the corrosion probability of stainless steels in different industrial and natural

environments. The proposed equations, which relate input parameters and transitional

probabilities were, initially, empirical expressions based on engineering knowledge of

corrosion behavior of stainless steels; aim of this thesis is to validate and confirm these

mathematical expressions: electrochemical tests (potentiostatic, potentiodynamic and linear

polarization resistance tests) were carried out and the experimental results, in addition of

literature corrosion data, were carefully elaborated in order to propose new revised

equations of Markov model.

INTRODUZIONE

2

INTRODUZIONE

Gli acciai inossidabili sono utilizzati negli impianti industriali per la loro elevata resistenza

a corrosione; tuttavia, in presenza di cloruri, possono essere soggetti a pericolose forme di

attacco localizzato come pitting e crevice. Nella corrosione per pitting si distinguono due

stadi: l’innesco del pit e la sua propagazione; poiché una volta innescato il pit propaga

velocemente, molte risorse sono state impiegate, sia in passato che nel presente, nel

tentativo di trovare modelli che permettano la previsione del tempo d’innesco; il pitting è

un fenomeno intrinsecamente stocastico, il cui innesco è caratterizzato da una variabilità

sia temporale che spaziale: la sua previsione deve essere effettuata, quindi, secondo un

approccio probabilistico. In questo scenario si inserisce la proposta di un modello

matematico che utilizza delle matrici di Markov per la previsione della probabilità

d’innesco del pitting e che risulta particolarmente utile per la classificazione della

resistenza a pitting dei diversi acciai inossidabili. Caratteristica di un processo stocastico

markoviano è l’assenza di memoria: la sua evoluzione temporale dipende, quindi, solo dal

suo stato attuale. Per la descrizione del fenomeno del pitting è stato proposto un modello a

catene di Markov a cinque stadi che prevede due stati assorbenti, quello di pitting e di

ripassivazione, e tre stati di transizione, quello matastabile, di metapitting e di

metapassività, come mostrato in figura.

Modello di Markov a 5 stadi.

Le probabilità r, m e p sono state inizialmente definite mediante relazioni empiriche in

funzione dell’acciaio inossidabile (PREN) e di parametri operativi, come contenuto di

INTRODUZIONE

3

cloruri, pH, temperatura, condizioni fluidodinamiche e potere ossidante del sistema, tarate

sulla base della conoscenza ingegneristica del comportamento degli acciai inossidabili.

Questo lavoro di tesi si propone l’obbiettivo di validare queste equazioni tramite

elaborazione di dati di letteratura ed esperimenti di laboratorio. Sono state effettuate delle

prove potenziostatiche con tre acciai inossidabili (PREN 17, 18 e 24) in diverse condizioni

definite dal potenziale di polarizzazione, dalla temperatura e dal contenuto di cloruri; le

prove hanno permesso di ottenere valori sperimentali di probabilità di corrosione che sono

stati confrontati con quelli previsti dal modello di Markov esistente: è stata osservata una

differenza rilevante tra i risultati di laboratorio e quelli del modello, soprattutto per le

condizioni sperimentali meno aggressive. Tenendo comunque sempre presente i limiti

delle prove di corrosione accelerate e la difficoltà dell’interpretazione dei loro risultati,

sono state effettuate prove elettrochimiche (potenziodinamiche e di polarizzazione lineare)

volte alla modifica delle equazioni della probabilità p e m: la struttura matematica del

modello e i fattori d’influenza delle probabilità sono rimasti invariati ma si sono apportate

delle modifiche nelle relazioni tra i parametri di input e le probabilità.

La tesi è strutturata in sei capitoli: nel primo viene descritto il fenomeno della corrosione

localizzata degli acciai inossidabili e i suoi fattori d’influenza; nel secondo si sottolinea

l’importanza dell’approccio probabilistico per la descrizione dello stadio d’innesco del

pitting e si propongono le equazioni esistenti del modello di Markov a cinque stadi; il terzo

capitolo descrive le prove di polarizzazione potenziostatica effettuate e propone, tramite

tabelle e istogrammi, il confronto tra le probabilità di corrosione sperimentali e quelle del

modello. Il capitolo quattro è incentrato sulla probabilità p: tramite la rielaborazione di dati

di letteratura sono proposte due nuove equazioni che vengono validate per mezzo di prove

sperimentali (potenziodinamiche). Nel capitolo cinque vengono descritte le prove di

polarizzazione lineare effettuate a diversi pH e temperature, i cui risultati, rielaborati,

permettono di modificare due delle equazioni che definiscono la probabilità m. Le nuove

equazioni delle probabilità p e m sono state quindi sostituite nel modello e le risultanti

probabilità di corrosione, calcolate tramite Matlab®, sono state confrontate nel capitolo sei

con quelle sperimentali e del vecchio modello.

Corrosion of stainless steel: an overview Chapter 1

4

Chapter 1

CORROSION OF STAINLESS STEEL: AN OVERVIEW

1.1 STAINLESS STEELS

Stainless steels are iron-chromium or iron-chromium-nickel alloys containing a minimum

of approximately 11% chromium; this amount of chromium allows the formation on the

metal surface of a thin protective oxide film (thickness in the order of 1 to 10 nm) which

reduces steel corrosion rate in several environments, as neutral electrolytes without

chlorides. In order to be protective from corrosion, the oxide film must be stable in the

environment where the metal works, it must be compact, uniform and non-porous over the

entire surface of the metal.

In addition to chromium, other alloying elements provide specific properties or ease of

fabrication. The most beneficial elements to increase corrosion resistance are chromium,

molybdenum, tungsten, nitrogen and nickel; otherwise, sulfur and manganese are

considered detrimental [1].

Commercial stainless steels are divided into three groups according to the metallurgical

structure: austenitic, ferritic and martensitic. The American Iron and Steel Institute (AISI)

designates standard grades of stainless steels by three digit numbers. The austenitic grades

are designated by codes in the 200 and 300 series, whereas the ferritic and martensitic

grades are designated in the 400 series. Duplex stainless steels, precipitation hardening

stainless steels and cast stainless steels are generally known by other designations [1].

The Schaeffler diagram (Fig.1.1) relates the metallurgical structure with the composition of

stainless steels, conveniently expressed in terms of either nickel equivalent (austenite

stabilizer) or chromium equivalent (ferrite stabilizer) on a weight percentage basis. It is not

an equilibrium diagram because it indicates the structure obtained after rapid cooling at

room temperature from 1050°C. The alloying elements commonly found in stainless steels

are divided either as austenite stabilizer (nickel, cobalt, carbon, nitrogen, manganese,

copper) or ferrite stabilizer (chromium, silicon, molybdenum, vanadium, aluminum,

niobium, titanium). Austenite stabilizers extend the γ-domain of the steel equilibrium

Corrosion of stainless steel: an overview Chapter 1

5

diagram, chromium, instead, acts by closing the γ-region increasing whose of ferrite.

However, when chromium is added to a steel containing nickel it retards the kinetics of the

γ → α transformation, thus making it easier to retain austenite at room temperature [1].

1.1.1 Austenitic stainless steels

As name suggests, austenitic stainless steels show an austenitic microstructure with a faced

centered cubic lattice. This structure makes them extremely formable and weldable; they

can be successfully used from cryogenic temperatures to the red-hot temperatures of

furnaces and jet engines. They contain chromium in the range from 16 to 25%, nickel in

the range of 5-15% and other elements in solution, as shown in Table 1.1. The addition of

molybdenum improves pitting and crevice corrosion resistance; a low carbon content

and/or the addition of titanium reduce intergranular corrosion in welded materials; nickel

and chromium are added to improve high temperature oxidation resistance, strength and

stress corrosion resistance [1].

Stainless steel type 304, the general purpose grade is widely used in applications requiring

a good combination of corrosion resistance and formability and is one studied in this work.

Figure 1.1- Schaeffler diagram [1].

Corrosion of stainless steel: an overview Chapter 1

6

Table 1.1- General chemical composition of austenitic stainless steels available on the market.

AISI

grade C % Mn % P % S % Si % Cr % Ni % Mo %

201 0,15 5,5 7,5 0,045 0,015 1 16 18 3,5 5,5 -

202 0,15 7,5 10,5 0,045 0,015 1 17 19 4 6 -

301 0,05 0,15 2 0,045 0,015 2 16 19 6 9,5 0,8

304 0,07 2 0,045 0,015 1 17 19,5 8 10,5 -

304L 0,03 2 0,045 0,015 1 18 20 10 12 -

316 0,07 2 0,045 0,015 1 16,5 18,5 10 13 2 2,5

316L 0,03 2 0,045 0,015 1 16,5 18,5 10 13 2 2,5

330 0,15 2 0,045 0,015 1 2 15 17 33 37 -

1.1.2 Ferritic stainless steels

Stainless steels with ferritic microstructure have a body centered cubic lattice structure:

they are less ductile than austenitic stainless steels and not hardenable by heat treatment as

martensitic steels; some examples are shown in Table 1.2. They resist corrosion and

oxidation and are also resistant to stress corrosion cracking; ferritic stainless steels are used

for decorative trim, sinks and automotive applications, particularly exhaust system. The

most popular ferritic grade is type 430, with a range of chromium content between 12 and

18%: a low chromium content (12-13%) improves weldability, impact resistance, strength

and hardness, but implies loss in corrosion resistance; an high chromium content (16-18%)

involves gain in corrosion resistance but loss in mechanical properties [1].

Table 1.2- General chemical composition of ferritic stainless steels available on the market.

AISI grade C % Mn % P % S % Si % Cr % Ni % Mo %

405 0,08 1,0 0,04 0,015 1 12 14 - -

409 0,03 1 0,04 0,015 1 10,5 12,5 0,3 1 -

430 0,08 1 0,04 0,015 1 16 18 - -

439 0,05 1 0,04 0,015 1 16 18 - -

446 0,15 0,2 1 0,04 0,015 1 26 29 - -

Corrosion of stainless steel: an overview Chapter 1

7

1.1.3 Martensitic stainless steels

Martensitc stainless steels have an austenitic structure at elevated temperatures which can

be transformed into martensite by a proper cooling (quenching) to room temperature. After

quenching they show a martensitic structure characterized by a body centered tetragonal

lattice, high hardness and mechanical strength. In martensitic stainless steels chromium lies

in the range from 11,5 to 18%, with the lower limit being governed by corrosion resistance

and the upper limit by the requirement for the alloy to convert fully to austenite during

heating. After rapid cooling, the steels hardened by transformation martensite must be

tempered (heated at a temperature such as to achieve hardness reduction) in order to obtain

mechanical properties suitable for engineering applications [2]. Martensitic grades (some

example in Table 1.3) are used when, in addition to moderate corrosion resistance,

hardness, strength and wear resistance are required, so for istance for turbine components,

valve parts, cutlery, fasteners and machinery parts.

Table 1.3- General chemical composition of martensitic stainless steels available on the market.

AISI grade C % Mn % P % S % Si % Cr % Ni % Mo %

403 0,08 0,15 1,5 0,04 0,015 1 11,5 13,5 0,75 -

416 0,08 0,15 1,5 0,04 0,015 0,025 1 12 13,5 - 0,6

420 0,16 0,25 1,5 0,04 0,015 1 12 14 - -

440A 0,65 0,75 1 0,04 0,015 0,70 14 16 - 0,5

1.1.4 Duplex stainless steels

Duplex stainless steels show a two-phases microstructure consisting of ferritic and

austenitic grains, roughly 50% austenite and 50% ferrite. Duplex stainless steels show a

mechanical strength which is twice higher than austenitic or ferritic stainless steels; they

have significantly better toughness and ductility than ferritic grades although they don’t

reach the excellent values of austenitic grades.

Duplex stainless steels also improved resistance to localized corrosion, particularly pitting,

crevice corrosion and stress corrosion cracking. They are characterized by high chromium

(up to 32%) and molybdenum (4-5%) and lower nickel contents than austenitic stainless

Corrosion of stainless steel: an overview Chapter 1

8

steels (Table 1.4). They are widely used in chemical process industry, not only in chlorides

containing environments, where they are more resistant to stress corrosion cracking than

austenitic grades, but also in strongly alkaline chlorides-bearing solution, in caustic fluids

and high temperature application.

Table 1.4- General chemical composition of duplex stainless steels available on the market.

AISI grade C % Mn % P % S % Si % Cr % Ni % Mo %

329 0,05 2 0,035 0,015 1 25 28 4,5 6,5 1,3 2

S31803 0,03 2 0,035 0,015 1 21 23 4,5 6,5 2,5-3

S32550 0,03 2 0,035 0,015 0,7 24 26 5,5 7,5 2,7 4

S32760 0,03 1 0,035 0,015 1 24 26 6 8 3 4

1.2 CORROSION FORMS OF STAINLESS STEEL

1.2.1 General corrosion

Uniform (or general) corrosion is a corrosion attack uniformly distributed over the entire

surface of a metal. Corrosion proceeds at approximately the same rate over the metal

surface. The material becomes thinner as it corrodes until its thickness is reduced to the

point at which failure occurs. Failures by general corrosion are less feared than those by

localized corrosion because they are more predictable [1].

Stainless steels can exhibit general corrosion in strong acids, as in chemical plants [1].

1.2.2 Localized corrosion

The most dangerous corrosion form of stainless steels is localized corrosion; it proceeds

corresponding to small areas on the metal surface in contact with a corrosive environment.

This corrosion form starts with the localized breakdown of the passive film corresponding

to surface defects of the metal (as inclusions, welding) or in correspondence of

heterogeneity of the electrolyte (area with higher temperature, higher concentration of

Corrosion of stainless steel: an overview Chapter 1

9

aggressive chemicals or with lower pH). Once the passive film is damaged, corrosion

propagates into the bulk material with high corrosion rate, up to some mm/year.

Pitting, crevice, stress corrosion cracking, corrosion fatigue and intergranular corrosion are

the most frequent causes of failure of stainless steel components.

This work will focus on pitting and crevice corrosion which will be described in the

following.

1.3 PITTING CORROSION

Pitting is a form of localized corrosive attack that leads to the creation of localized anodic

area (pits) on the metal surface (Fig. 1.2); due to the high corrosion rate corresponding to

the formed pits, their depth can affect in a short time the whole thickness of metal walls

[4]. As every localized corrosion form, pitting is considered detrimental for the engineering

use of stainless steels and must be correctly prevented.

Figure 1.2- Typical shape of pitting corrosion attack [4].

1.3.1 Pitting corrosion mechanism

Pitting corrosion attack can be divided in two stages: initiation and propagation. Pitting

initiation is related to interaction between chloride ions and the passive film, whose

inclusions, second phases and areas of compositional heterogeneity, which are always

present in commercially produced stainless steels, are preferential sites for pits nucleation;

pits may also nucleate in regions where the environment is more aggressive, due, for

example, to temperature or chlorides concentration increase or pH decrease [4].

Corrosion of stainless steel: an overview Chapter 1

10

The pit propagation process is illustrated schematically in Fig.1.3 for a stainless steel in

neutral aerated sodium chloride solution.

Figure 1.3- Pitting corrosion attack mechanism [4].

Once pits are initiated they may continue to grow by a self sustaining mechanism [1]: pit

propagation involves the creation of a macrocouple current between the anodic area (pit),

where dissolution of the metal occurs (M M+ + e

-), and the cathodic area (adjacent

metal), where oxygen reduction occurs (O2 + 2H2O + 4e-

4OH

-). The anodic current

density can be very high compared to the cathodic one, because the ratio between cathodic

area and anodic area can also reach values higher than 1000 [4]: then, to gain electrons

balance, the anodic current must be much greater than the cathodic one.

During propagation stage, the solution inside the pit becomes gradually more aggressive

due to the hydrolysis reactions of metal ions (Mz+

+ zH2O → M(OH)z + zH+), which

determine a progressive acidification; meanwhile, the pH of the bulk solution remains

neutral or increases thank to cathodic oxygen reduction. Furthermore, the circulation of the

macrocouple current favors the increase of chlorides ions concentration within the pit [4].

Consequently, pitting corrosion attack propagates with increasing speed (autocatalytic

mechanism) and does not tend to spread to the surface of the material, but to penetrate

inside. Corrosion rate can reach high values, in many cases of the order of few millimeters

per year [4].

Corrosion of stainless steel: an overview Chapter 1

11

1.3.2 Thermodynamic and kinetic aspects of pitting corrosion

In order to understand the thermodynamic corrosion behavior of stainless steels, the

chromium potential-pH diagram (Pourbaix diagram) should be considered. Pourbaix

diagram enables the determination of condition (pH and potential intervals) for immunity,

where no corrosion is possible, passivation, where a corrosion product film forms and may

confer protection against corrosion, and for corrosion, where corrosion is expected [2].

Figure 1.4 shows chromium Pourbaix diagram, main element of the stainless steel

protective film: in a large range of pH (neutral and passive) and potential, the protective

chromium oxides film, which lowers stainless steel corrosion rate to negligible values, is

stable. As already explained, passive film stability decreases in chlorides containing

environment; Figure 1.5 shows chromium Pourbaix diagram in solutions containing

chlorides: the stability region of chromium oxide in dramatically reduced.

Fig. 1.4- Chromium Pourbaix diagram [5]. Fig. 1.5- Chromium Pourbaix diagram in

solution containing chlorides [5].

Corrosion of stainless steel: an overview Chapter 1

12

Fig. 1.6- Evan’s diagram: anodic curve of a passive metal and cathodic curve (red line) arising

from oxidizing condition.

Passivity of stainless steels can be studied by means of the potential-current curves (Evan’s

diagram) which represent cathodic and anodic partial reactions constituting the overall

corrosion process. Figure 1.6 shows the intersection of the anodic curve of stainless steel

and the cathodic curve resulting from oxidizing condition. The intersection point defines

the corrosion potential Ecorr and the corrosion current icorr.

Figure 1.7 shows the general features of a passive material (as stainless steel) anodic curve:

the current initially increases with an increase in potential until the potential reaches Ep

(passivating potential); the current density than decreases markedly to the passive current

density ip, signaling the onset of passivity. When the potential reaches the value Ebd

(breakdown potential or pitting potential) the current density increases above ip and

corrosion starts [2]. In the transpassive region oxygen evolution and possibly increased

corrosion is observed. It’s important to point out that, at potentials far below Ebd, and

during the induction time before the onset of stable pitting at potentials above the pitting

potential, metastable pits can form; metastable pits are pits that initiate and grow for a

limited period before repassivating: they are typically considered to be those of µm size at

most with a lifetime on the order of seconds or less [6]. The effect of chloride ions on the

anodic curve of stainless steel (section 1.3.6) is that of reducing pitting potential and then

the passivity region (Fig.1.8).

Corrosion of stainless steel: an overview Chapter 1

13

Fig. 1.7- Anodic curve of stainless steel. Fig. 1.8- Effect of chlorides of anodic curve of

stainless steel.

Another anodic curve feature of great interest is the repassivation potential, Erp (or

protection potential, Eprot), shown in Figure 1.9. In general, once initiated, localized

corrosion sites can propagate only at some potential more positive than the protection

potential [7] ; in other words, even after pitting initiation, repassivation will occur at more

negative potential. Therefore, the more positive Eprot is, the less likely localized corrosion

will propagate. At potential between Ebd and Eprot, sites that have initiated can propagate.

The Pedeferri diagram (Fig.1.10) shows conditions for immunity, passivity and corrosion

in terms of chlorides concentration and potential and is commonly used to evaluate

initiation condition of reinforced concrete in presence of chlorides. Carbon steel rebars are

passive because concrete pH is around 12; but, if the chloride concentration reaches the

critical threshold, pitting corrosion can start. In the Pedeferri diagram four regions can be

identified [4]: the region A is characterized by the conditions that cause the initiation and

propagation of the pit; region B provides the conditions that do not allow new pit initiation,

but only the propagation of those already started; region C gives the conditions which

allow neither the initiation of new pits nor the propagation of already started pits; region D

determines the immunity conditions.

Corrosion of stainless steel: an overview Chapter 1

14

Figure 1.9- Anodic curve of a passive metal: pitting and repassivation potential definition [4].

Figure 1.10- Pedeferri diagram [4].

1.3.3 Effect of stainless steels composition on pitting resistance

The corrosion resistance of stainless steels can be increased by modification of the

chemical composition of the alloy by introducing some metallic or non metallic elements

which improve the corrosion behavior [4]. Generally, alloying elements increase the ability

of the metal to form a stable and resistant passive film. Figure 1.11 summarizes the effect

of some alloying elements on the anodic curve of stainless steel. In particular, the presence

of chromium shifts Epitt towards more noble value and ic, ip, which are a measure of the

susceptibility to passivation, towards lower values [8]; the addition of molybdenum

Corrosion of stainless steel: an overview Chapter 1

15

increases the strength of the passive film; nitrogen increases corrosion resistance of

austenitic stainless steels but can be detrimental for ferritic grade; nickel, although does not

interfere with pitting initiation, slows the propagation and favors the repassivation.

Niobium and titanium are “stabilizers” because they are able to prevent sensitization

phenomena and intergranular corrosion. Otherwise, manganese is affine to sulfur and tends

to form sulfides which are sites for pits initiation [9]. Boron, carbon and copper can have a

variable effect. Boron is beneficial if it is in solid solution, but detrimental when

precipitated as intermetallic compound. Carbon has no effect on pitting resistance if it is in

solid solution but is detrimental when precipitated as carbide. Copper has no effect in the

absence of molybdenum, but a slightly detrimental effect in its presence [1].

Figure 1.11- Effect of some alloying elements on the anodic polarization curve of stainless steel

(adapted from [10]).

The effect of stainless steel composition on pitting corrosion resistance is commonly

described by means of the “Pitting Resistance Equivalent Number” (PREN) which takes

into account chromium, molybdenum, tungsten and nitrogen concentration by the formula:

Eq. 1.1

With X=0 for ferritic stainless steels, X=16 for austenitc and X=30 for duplex stainless

steels [11].

Corrosion of stainless steel: an overview Chapter 1

16

This index is used to rank and compare the pitting corrosion resistance of different types

of stainless steels. In general the higher is the PREN, the higher will be the chloride

concentration tolerable in the solution, the higher will be the breakdown potential [4].

Figure 1.12, 1.13 and 1.14 show the effect of Cr, Mo and Ni, respectively, on pitting

potential of different stainless steels in 0,1 N NaCl solution at 25°C (3500 ppm Cl-).

Figure 1.12- Effect of chromium content on

pitting potential of iron-chromium alloys in

deareated 0.1 N NaCl solution at 25 °C [1].

Figure 1.13- Effect of molybdenum content on

pitting potential of Fe-15% Cr-13% Ni alloys in

a deareated 0.1 N NaCl solution at 25°C [1].

As already explained in section 1.1, a chromium content lower than 12% is not enough to

form a stable passive film on the metal surface. Increasing chromium content, stainless

steel pitting resistance improves: as shown in Fig. 1.12, up to 20% there is only a small

variation of the pitting potential which, instead, increases dramatically for chromium

concentration between 25 and 35% and stabilizes to noble value for high chromium

content. As shown in Fig. 1.13, the effect of molybdenum content on stainless steel pitting

potential is quite strong: molybdenum weight percentage variation from 1 to 2% involves

an increase of 200 mV of the pitting potential. The increase of nickel content also improves

pitting corrosion resistance, but less dramatically: in particular, as shown in Fig.1.14, every

10% increase of nickel content involves an increase of 5 mV of stainless steel pitting

potential.

Corrosion of stainless steel: an overview Chapter 1

17

Figure 1.14- Effect of nickel content on pitting potential of Fe-15% Cr alloys in a deareated 0.1 N

NaCl solution at 25 °C [1].

Figure 1.15- Effect of PREN on pitting potential of stainless steel in a 0.6 M NaCl solution at

25°C (21000 ppm Cl-). [3]

Figure 1.15 displays the relationship between pitting potential and PREN. Pitting potential

increases linearly as PREN increases up to 30, then sharply reaches values of the order of 1

V SCE and stabilizes for PREN higher than 35. It is worth to point out the statistical

distribution of pitting potential due to the intrinsic stochastic nature of pitting corrosion

(see section 2.1) and to the fact that stainless steels with different chemical composition

have the same PREN.

Corrosion of stainless steel: an overview Chapter 1

18

1.3.4 Effect of microstructure on pitting behavior of stainless steel

Steel microstructure plays an important role in determining pitting resistance. Phases such

as sulfides, δ-ferrite, α-prime, σ-phase, the strengthening precipitates in precipitation

hardening stainless steels, sensitized grain boundaries, and welds, can have an effect on

pitting resistance [1].

Studies of the role of manganese sulfide inclusions in the pitting behavior of stainless

steels have led to a recognition of the importance of the composition of these inclusions:

high chromium content manganese sulfide inclusions could improve pitting resistance [1].

δ-ferrite in austenitic stainless steels is generally considered detrimental to pitting

resistance; σ-phase is also detrimental, even if it contains higher chromium and

molybdenum than the austenitic matrix and exhibits more noble potential in chloride

solutions than austenite: some chromium or molybdenum depletion is occurring within the

austenite immediately adjacent to the precipitating sigma, and the pits sites may be

associated with such depleted region [1], as in intergranular corrosion form.

1.3.5 Effect of surface finish on pitting behavior of stainless steel

A factor in determining pitting potential for a given alloy/environment system is the

surface finish of the material. Comparing the pitting tendencies of different alloy having

different surface finishes can yield non significant results [1]. Anyway, the consensus is

that smoother surfaces have higher pitting resistance than rough surfaces [12,13]: peaks

and valley structure of rough surfaces makes easy the chloride ions accumulation;

furthermore, surface defects and discontinuity may act as preferential site for pits initiation

or play the role of crevice. Among chemical surface treatments aimed at improving pitting

resistance, “passivation” is a well known one and consists of immersing the stainless steel

in a 20% HNO3 solution [1,12]. The main effect of this treatment is to clean the stainless

steel by dissolving surface inclusions and contaminants, such iron and steels particles

embedded in the surface during fabrication. This treatment also removes from the surface

manganese sulfide particles which can act as pit initiation sites.

Corrosion of stainless steel: an overview Chapter 1

19

1.3.6 Effect of environmental parameters on pitting resistance of stainless steel

From a practical viewpoint most equipment failures due to pitting corrosion are caused by

chloride and chlorine containing ions [1]. In general, whatever the conditions considered,

the presence of chloride ions tends to promote the passive film breakdown. Increasing the

chloride concentration of a solution significantly increases pitting corrosion probability.

The effect of chloride ions on the anodic curve of stainless steel, shown in Fig.1.16, are the

decrease of pitting potential and the increase of the passivity current. Figure 1.17 shows the

decrease of pitting potential of AISI 316 and 304 stainless steels as chlorides content of the

solution increase. For example, the pitting potential of AISI 304 goes from 200 mV SCE at

3500 ppm Cl- to -200 mV SCE at 35000 ppm Cl

-.

Figure 1.16- Effect of chloride ions on the

polarization curve of stainless steel [2].

Figure 1.17- Effect of chlorides

concentration on the pitting potential of AISI

316 and 304 at room temperature in a 3%

NaCl solution [1].

The effect of temperature on pitting corrosion resistance is reported in Figure 1.18: pitting

potential decreases by increasing the temperature. Nevertheless, the effect of temperature

on pitting potential also depends on the composition of the alloy [1]: as seen from Fig.

Corrosion of stainless steel: an overview Chapter 1

20

1.18, for the molybdenum containing type AISI 316 at temperature above 70°C, the pitting

potentials become largely independent of temperature.

Figure 1.19 shows the relationship between stainless steels pitting potential and the pH of

the solution: pitting potential increases slightly with pH up to pH 8 when a stronger passive

film forms. Thus, at low pH stainless steels approach the region of active corrosion

indicated in Pourbaix diagrams where the stability of the passive layers are reduced; on the

contrary, an increase in the pH value favors the existence of more stable passive films, and

therefore, the pitting potential increases and the corrosion rates lowers [14].

Figure 1.18- Effect of temperature on the pitting

potential of various stainless steels in a 3% NaCl

solution. [1]

Figure 1.19-Effect of pH on pitting potential of

various stainless steels in a 3% NaCl solution.

[1]

Also solution velocity has an effect on pitting corrosion resistance of stainless steels [1].

Pit initiation is more difficult in fluids with higher flow velocities and pit is suppressed by

increasing flow velocity in the turbulent regime [15]. At sufficiently high velocity the

chemical species within the pit are dislodged from the pit thus interfering with the growth

of metastable pit and ultimately hindering stable pit formation. The pitting potential is then

shifted in the noble direction and the pit formation is suppressed [15].

Corrosion of stainless steel: an overview Chapter 1

21

1.4 CREVICE CORROSION

Crevice corrosion is a form of localized corrosion that may occur within crevices or at

shielded surfaces where a stagnant solution is present [1]. The crevice must be wide

enough to permit the solution to enter, but sufficiently narrow to maintain a stagnant zone

of solution within the crevice so that the removal of the reaction products is very slow and

occurs only by diffusion and migration [11].

Such crevices may be formed by the geometry of the structure, e.g. gaskets, rivets, welded

fabrications, threaded joints; crevices can also arise from the contact between the metal and

non-metallic solids, e.g. plastics, rubber, glass. Corrosion can also take place under

deposits of sand, dirt or permeable corrosion products on the metal surface (under deposit

corrosion) [11].

Figure 1.20- Crevice corrosion: (a) crevice resulting from the joining of the two plates of steel; (b)

crevice due to a gasket between two flanged pipes [11].

Crevice corrosion mechanism for a stainless steel in an aerated sodium chloride solution is

very similar to that proposed for pitting [1]. The main difference is that the location of a

possible crevice corrosion initiation is predictable: the obvious method of controlling

crevice corrosion is to avoid crevices in the design of the structure, or at least to keep them

as open as possible, and to avoid geometrical conditions that lead to the formation of

deposits on the metal surface.

Corrosion of stainless steel: an overview Chapter 1

22

Figure 1.21 is a schematic illustration of the crevice corrosion mechanism: initially anodic

and cathodic reactions take place uniformly over the entire metal surface, including the

surface within the crevice. Nevertheless, inside the crevice the oxygen consumed by the

cathodic reaction is not replenished with the subsequent formation of an occluded cell

where oxygen concentration is lower than outside the crevice. The anodic process occurs

inside the crevice but the cathodic reactions only outside, where oxygen is present: the

high ratio beween cathodic and anodic area involves an high corrosion rate. The current

flowing between the anodic and cathodic areas leads to an increase of the chlorides

concentration in the crevice [4]. At the same time, metal ions hydrolysis results in a sharp

drop in pH. When the acidity and the chlorides concentration reach a critical threshold,

which depends on the stainless steel corrosion resistance, there is the breakdown of the

passive film. At this point begins the propagation phase: in a first time, corrosion rate

increases because current circulation between anodic and cathodic areas makes the

environment inside the crevice more aggressive. The growth then ceases when the current

reaches a value such that the ohmic drop consumes all the work available for the

occurrence of the process [4].

Figure 1.21- Schematic illustration of the crevice corrosion mechanism [1].

As regard stainless steels, the major alloying elements, nickel and chromium, increase

resistance to crevice corrosion; the beneficial effect is attributable to the fact that

chromium and nickel rise the pitting potential of the material in the more noble direction.

Another important alloying element which increase crevice resistance of stainless steels is

molybdenum which increases difficulty in breaking down the passive film and raises Epitt

in the noble direction [11].

Corrosion of stainless steel: an overview Chapter 1

23

ASTM G48 and ASTM G78 cover procedures for the determination of the resistance of

stainless steels crevice corrosion when exposed to oxidizing chloride environments and

provide a basis for assessing the relative resistance of various alloys to crevice corrosion

under certain specified conditions. Also in the case of crevice corrosion the PREN index

(Eq. 1.1) is used to rank stainless steels; at equal environmental conditions, in order to

prevent crevice corrosion, stainless steels with higher PREN than that used to prevent

pitting corrosion are needed [8].

For the elaboration of the Markov model used in this work of thesis, the crevice is simply

considered a more aggressive form of pitting [16]; if the stainless steel is immersed in an

environment particularly narrow and aggressive, the corrosion phenomena is more critic

and occurs as crevice corrosion.

Markov model: state of art Chapter 2

24

Chapter 2

MARKOV MODEL: STATE OF ART

2.1 INTRODUCTION

Pitting corrosion is a stochastic phenomenon and its initiation is characterized by an

intrinsic variability [17]. It follows that pitting corrosion cannot be explained without

statistical and stochastic methods [18]: the experimental data concerning the occurrence of

pitting corrosion (initiation time, corrosion current, pitting potential), obtained from a set

of measurements under the same experimental or field conditions, are scattered for a given

metal [19]. The breakdown potential, for example, is typically observed to be a

significantly “statistically distributed” property [7, 13, 19, 20]. These distribution have

been attributed to the stochastic nature of pitting [7] and to the inherent randomness of the

corrosion system [21]. From a microstrustural point of view, metals are generally

polycrystalline materials consisting of grains of different forms and orientations, on the

boundaries of which various chemical elements are concentrated. In addition, cracks,

inclusions, voids, etc., occur within metals. These microstructural features cause metals to

be susceptible to random variations in physical properties and, consequently, in their

corrosion behavior. Likewise, local variations in flow conditions, temperature, pH, etc., are

some of the environmental parameters to be considered. Thus the inherent randomness of

the corrosion system can be viewed from the high degree of complexity of the metal-

protection-environment combination [21].

Anyway, it is important to be able to determine the extent of pitting, either to select the

most pitting-resistant materials for service, or to predict the remaining life of a metal

structure [22]. Then, the two stages of pitting (initiation and propagation) must be

considered: probabilistic methods for prediction of initiation time and propagation time

have been developed in the last decades. ASTM G16 and G46 standardize statistical

analysis of pitting corrosion data, as, for example, extreme value statistics (section 2.5), or

methods to rate pits in terms of density, size, and depth as, for example, standard charts

(Fig. 2.1).

Markov model: state of art Chapter 2

25

Figure 2.1- Standard rating charts for pits [22].

From an engineering point of view it’s of practical interest the prediction of the initiation

time, because, once pit starts, its propagation is very fast and generally unstoppable; the

major effort, then, must be focused on materials selection and plants design and

maintenance. An analytic method to evaluate system reliability, or, in other words, to

calculate corrosion probability, is a stochastic model based on Markov chains [23]: a five-

steps Markov model for pitting prediction is described in the following sections of the

chapter.

2.2 MARKOV CHAINS

In this thesis the pitting corrosion phenomena is described by a Markov process which

assumes that pitting corrosion retains no memory of the past, so only the current state of

the damage influences its future development [24]. Some basics of Markov chains

mathematical concepts follow.

Markov model: state of art Chapter 2

26

A stochastic process is a phenomenon that varies to some degree unpredictably as time

goes on [25]. In defining such a process it is necessary to specify the time set T involved,

that can be continuous (Eq. 2.1) or discrete (Eq. 2.2):

Eq. 2.1 0 t:t T

Eq. 2.2 ... 3, 2, 1, 0,T

Suppose that at each point of the time set T, a measure of the random variable X can be

observed. Thus, a given experiment is assumed and for each sample point or experimental

outcome there corresponds not a single number but an entire function Xt. If the sample

point or the outcome is denoted by x, this function can be properly denoted by

. The probability structure of the stochastic process is completely defined

provided that the probability density function of this set of variable is determined.

Basically, the analysis of a stochastic process involves determining the density function,

, and using it to predict the behavior of the process in the future, given

a certain behavior in the past [25].

Classes of stochastic process can be defined by imposing suitable restriction on the n-

dimensional density function [25]:

Stationary processes: their probability density functions are invariant to time translation.

Gaussian, or normal, processes: their density functions are multivariate normal.

Markov processes: their density functions are function only of the immediate past of the

story and not of its entire history.

A Markov chain is a system which starts in one of the states defined by Eq. 2.3 and

successively moves from one state to another [26]; each move is called a step.

Eq. 2.3 k321 s ..., ,s ,s,sT

Markov model: state of art Chapter 2

27

The probability pij(n) that the chain from the state si moves to state sj at the next step does

not depend upon which states the chain was in before the current state. The probabilities

pij(n) are called transition probabilities. The process can remain in the state it is in, and this

occurs with probability pii. An initial probability distribution, denoted on S, specifies the

starting state. Usually this is done by specifying a particular state as the starting state [26].

Let P be the transition matrix of a Markov chain, its ijth

entry pij(n)

gives the probability that

the Markov chain, starting in state si, will be in state sj after n steps.

Consider, now, the long-term behavior of a Markov chain when it starts in a state chosen

by a probability distribution on the set of states, which is called a probability vector. If u0

is a probability vector which represents the initial state of a Markov chain, the ith

component of u0 represents the probability that the chain starts in state si.

Let Pn be the transition matrix of a Markov chain, and let u0 be the probability vector

which represents the starting distribution. Then the probability that the chain is in state si

after n steps is the ith

entry in the vector [26]:

Eq. 2.4 n

0n Puu

As depicted in Equation 2.4, the transition matrix and its powers are the keys to define the

whole Markov process, knowing the initial probability distribution.

The Chapman-Kolmogrov equation is always valid for a Markov process; let be Pij(n) the

probability that the system go from si to sj in n steps, for r < n [26]:

Eq. 2.5 rnPrPP kjk ikij

The Chapman-Kolmogrov equation involves a new condition that the transition

probabilities must satisfy:

Eq. 2.6

A state si of a Markov chain is called absorbing if it is impossible to go away from it (i.e.,

pii = 1). A Markov chain is absorbing if it has at least one absorbing state, and if from

Markov model: state of art Chapter 2

28

every state it is possible to go to an absorbing state (not necessarily in one step). In an

absorbing Markov chain, a state which is not absorbing is called transient [26].

Consider an arbitrary absorbing Markov chain. Renumber the states so that the transient

states come first. If there are r absorbing states and t transient states, the transition matrix

will have the following canonical form [26]:

Eq. 2.7

Id

R

0

QP

Here Id is an r-by-r identity matrix which represents the probability to move from an

absorbing state to another, 0 is an r-by-t zero matrix because the probability to go from an

absorbing state to a transient state is zero, R is a nonzero t-by-r matrix which represents the

probability to move from a transient state to an absorbing one, and Q is an t-by-t matrix

which includes all the transition probabilities from a transient state to another [16].

As discussed before, the entry pij(n) of the matrix P(n)

is the probability of being in the state

sj after n steps, when the chain is started in state si. A standard matrix algebra argument

shows that P(n)

is of the form [34]:

Eq. 2.8

Id0

QP

n

n

Where the asterisk * stands for the t-by-r matrix in the upper right-hand corner of Pn:

Eq. 2.9 RQId1n

1k

k

The form of Pn shows that the entries of Q

n give the probabilities for being in each of the

transient states after n steps for each possible transient starting state. The probability of

being in the transient states after n steps approaches zero. Thus every entry of Qn must

approach zero as n approaches infinity (i.e, Qn 0). In other words, in an absorbing

Markov chain, the probability that the process will be absorbed is 1 (i.e. Qn 0 as n1)

[26].

Markov model: state of art Chapter 2

29

For an absorbing Markov chain P the matrix Id-Q has an inverse N and N = I + Q + Q2+…

is called the fundamental matrix for P. The ij-entry nij of the matrix N is the expected

number of times the chain is in the transient state sj, given that it starts in state transient

state si [26].

Let ti be the expected number of steps before the chain is absorbed, given that the chain

starts in state si, and let t be the column vector whose ith

entry is ti. Then,

Eq. 2.10 cNt

Where c is a column vector all of whose entries are 1.

Eq. 2.11

1

...

1

1

N

t

...

t

t

t

3

2

1

Let bij be the probability that an absorbing chain will be absorbed in the absorbing state sj if

it starts in the transient state si. Let B be the matrix with entries bij . Then B is an t-by-r

matrix [26]:

Eq. 2.12 RNB

where N is the fundamental matrix and R is as in the canonical form.

Knowing the expressions of the quantities calculated in the previous equations, the

computation of the probability distribution vector un can be performed by computer

programs, like MATLAB®, imposing a reasonably big number of steps n.

Markov model: state of art Chapter 2

30

2.3 THREE STEPS MARKOV MODEL

As already pointed out, a statistical approach is mandatory for the material selection in

engineering application due to the stochastic nature of pitting phenomenon and to the

several feature that affect pitting corrosion (initiation and propagation). In recent years,

important advances have been made in modeling pitting corrosion through Markov

processes: Rodriguez in 1986 [25] and Provan and Rodriguez [21] used a non-homogenous

Markov process to model pit depth growth for the first time; Hong [27] proposed a model

in which the pit generation process is represent by the Poisson process, and the pit depth

growth process by the Markov process; Valor et al. [28, 29] proposed a new stochastic

model in which pit initiation is modeled as a Weibull process, while pit growth is modeled

using a non-homogenous, linear growth Markov process.

The issue of all these models is the difficulty in the correlation of their specific parameters

with environmental, geometrical and metallurgical factors of real corrosion systems [30].

With the aim of proposing a model for practical application, Lazzari, Bolzoni et al. [30, 31]

used a continuous-time, three-state Markov process (Fig. 2.2) to model the first stages of

localized corrosion considering three possible states of the metal surface: two absorbing

states, passivity and localized corrosion, and one transient state, metastability. The

passivity state is characterized by a very small current density, the metastability by

oxidation phenomena of short duration (a few seconds to some minutes), and the localized

corrosion state by the formation of stable occluded cells.

Figure 2.2- Schematization of the three steps Markov model.

Markov model: state of art Chapter 2

31

The three states model has been resulted to be too simple and not adequate in describing a

lot of corrosion systems because not able to deal with conditions, for example, of

turbulence of the fluid, of cathodic protected system, of presence of biofilms or oxidizing

species [16]; a five step model has been then developed [16] and in this work of thesis an

attempt to validate it is moved.

2.4 FIVE STEPS MARKOV MODEL

Generally, the pitting corrosion phenomenon can be represented by a Markov process with

two absorbing states [16]: the pitting state, characterized by the formation of occluded

cells, and the passive state characterized by small corrosion currents. Thus, after a finite

but reasonably high number of transitions, the system will be absorbed necessarily by one

of these two states. The higher the probability to move to the passive absorbing state, the

higher the tendency of the material to resist pitting corrosion.

Three transient states, called metastability, metapitting and metapassivity, are defined to

take into account the presence of instability phenomena, the metastable pits formation and

repassivation [16]: indeed, before moving to an absorbing state, a passive metal as stainless

steel is generally subjected to micro-breakdown of the passive film which could, in a short

time, repassivate, or lead to pits formation.

In the five steps Markov model, represented in Fig. 2.3, the system, from the metastable

condition (initial condition), moves to an absorbing state step by step and with a defined

probability.

Figure 2.3- Schematization of the five steps Markov model.

Markov model: state of art Chapter 2

32

The initial state is the metastable state from which the system has a probability to move to

the metapassive condition (probability m) and to the metapitting state (probability 1-m).

The metapassive state shows a probability r to be absorbed by the passive state and 1-r to

go back to the metastable state; at the same time, the metapitting state has probability p to

move to pitting and 1-p to revert to the metastable condition. The probability m, r and p are

logically independent from each other [16].

The transition matrix (Eq. 2.13) and the distribution vectors (Eq. 2.14 and 2.15) are

expressed by:

Eq. 2.13

1

0

0

0

0

0

1

0

0

0

1

0

1

0

0

0

0

0

0

0

0

1

P

p

m

p

r

m

r

Eq. 2.14

0

0

1

0

0

u 0 Eq. 2.15

R

R

1

0

0

0

u n

Where R is the repassivation probability and 1-R the final corrosion probability.

Some considerations to discuss the transitional probabilities should be done. The

introduction of the metapassive and the metapitting states, with respect to the three steps

model, lead to the tendency of the final distribution vector to the passive state (if r

increases) or to the pitting condition (if p increases). If p is equal to r, the five steps model

becomes identical to the three steps one. If the initial state is the metastability and if m is

equal to 0,5, the final distribution vector would depend only on the ratio between p and r .

In the case that a transitional probability is zero, the system would not evolve to the

subsequent step: if p is zero, with r and m between 0 and 1, it would be impossible to have

pitting. Vice versa, if p is equal to one, once the system is in the metapitting condition, it

would evolve to pitting; but, considering that the starting condition is the metastable one

(Fig. 2.3), the system has some probability not to move to metapitting and can repassivate.

Markov model: state of art Chapter 2

33

The same reasoning remains valid for the r probability. If m will be equal to zero (or to

one), the passive state (or the pitting state) would be impossible to reach.

2.4.1 Transitional probabilities relation with input parameters

In order to obtain R and 1-R probabilities (Eq. 2.15), needed for Markov model practical

applications, the mathematical expressions of transitional probabilities r, m and p, and their

relations with pitting corrosion influence factors, are required.

Environmental, geometrical and metallurgical parameters which affect pitting corrosion

behavior of stainless steels are the following:

Chlorides concentration

Temperature

pH

PREN

Fluidodynamic condition of the system

Oxidant power of the system

Figure 2.4 shows the influence of these factors on the transitional probabilities. The m

probability depends mainly on the ratio between the solution chloride concentration and

critical chloride concentration for the material. As discussed before, if p is zero, pitting

would be avoided: this condition occurs only under cathodic protection condition and the

probability p then depends on the difference between the potential of the material in a

specific environment and the protection potential. The probability r expresses the tendency

of the system to repassivate and is considered dependent on the PREN and on the system

fluidodynamic condition.

On the basis of experimental results and corrosion engineering experience, equations,

which relates these parameters to transitional probabilities, have been proposed and

discussed in the following sections.

Markov model: state of art Chapter 2

34

Figure 2.4- Scheme of the influence factors of the transitional probabilities.

2.4.2 Transitional probability m: meta-stable to meta-passive transition

The transitional probability m is the probability that a stainless steel in a specific

environment moves from the initial state of metastability to the condition of metapassivity.

This probability depends on the factor k, defined as the ratio between the chlorides

concentration in the solution [Cl-] and the critical chloride threshold [Cl

-]cr. This

dependence, expressed by Eq. 2.16, is an exponential one, as shown in Figure 2.5: if the

chlorides concentration of the solution increases, the pitting susceptibility of stainless steel

also increases (see section 1.3.6): the repassivation probability will decrease.

Eq. 2.16

km

8,2exp1

Eq. 2.17 crCl

Clk

In particular, two cases can be well recognized:

When [Cl-]< [Cl

-]cr or k<1, m-probability tends to one: the material tends to

repassivate.

Markov model: state of art Chapter 2

35

When [Cl-]> [Cl

-]cr or k>1, m-probability rapidly decreases because the

environment becomes more aggressive; in particular, for k>10 m-probability

becomes rapidly less than 20%

Figure 2.5- k dependence of m-probability.

The concept of critical chloride content is widespread, for instance, in the study of

reinforced concrete structure: corrosion initiates corresponding to a critical chlorides

content reached at carbon steel rebar surface (in the range from 0,4 to 1% vs. cement in

aerated concrete); the main difficulty is that this parameter is not a unique value and

depends on several variables [32].

At the same way the breakdown of the passive film of stainless steel is more likely to occur

as the chloride concentration of the solution approaches the critical chloride content.

Equation 2.18 shows the relationship between the critical chloride threshold and

metallurgical, environmental and geometrical factors:

Eq. 2.18

crevice

crevice

cr k

k

TpHPRENClLog 3,0

4

1120

20

5,3

7

9

Markov model: state of art Chapter 2

36

As shown in paragraph 1.3.3, it is common to describe the pitting corrosion resistance of

stainless steel in terms of PREN. Materials with higher PREN are less susceptible to pitting

and can tolerate higher chloride concentration than lower PREN stainless steels, because

they have a stronger protective film. In corrosion engineering it is widespread the use of

the equation:

Eq. 2.19 9

PRENClLog cr

Where PREN depends on the chemical composition of the metal (Eq. 1.1)

Increasing the solution pH, the critical chloride thershold increases: an increase of the pH

favors the existence of more stable passive films, and therefore, the pitting resistance

increases; on the contrary, increasing the acidity of the electrolyte, materials approach the

region of active corrosion indicated in Pourbaix diagrams where the stability of the passive

layers are reduced. It has been chosen the value pH=2 as the limit under which stainless

steels will be subjected to general corrosion. The relation between the critical chlorides

threshold and pH (Eq. 2.20) is linear in semi-logarithmic scale as shown in Fig. 2.6.

Eq. 2.20 5,3

7 pH

ClLog cr

It’s worth to point out that the contribution of Eq. 2.20 to Eq. 2.18 becomes zero at neutral

pH. Figure 2.6 shows some theoretical curves obtained by using Eq. 2.20 for different

stainless steels (PREN from 18 to 40) at 20°C. At pH 7 the critical chlorides content for

AISI 304 is 100 ppm which decreases of an order of magnitude at pH 3. A PREN 40

duplex stainless steel has a critical threshold of about 30000 ppm at pH 7 which increases

up to 300000 ppm at pH 14.

Markov model: state of art Chapter 2

37

Figure 2.6- Critical chlorides threshold dependence of pH.

As widely known, the pitting corrosion resistance decreases by increasing temperature: the

kinetic of electrochemical reactions is faster and the material more susceptible to pitting

corrosion. Also the relation between critical chloride threshold and temperature is linear in

semi-logarithmic scale:

Eq. 2.21 20

20 TClLog cr

Also in this case, at room temperature the contribution of Eq. 2.21 to Eq. 2.18 is zero.

Indeed, at 20°C the critical chlorides content for AISI 304 is 100 ppm; raising the

temperature up to 40°C the critical threshold becomes 10 ppm.

The effect of system geometry is taken into account in equation 2.22 by a correction factor

equal to 1 in the presence of discontinuity, gaskets and any crevices on the metal surface; if

only pitting corrosion is expected kcrevice is equal to 0. Fig. 2.7 shows the temperature-

critical chlorides concentration trend and the effect of crevice: for example, the critical

threshold for AISI 316 at 40°C is about 60 ppm which decreases to 30 ppm in the presence

of crevices.

Markov model: state of art Chapter 2

38

Eq. 2.22 )25,01(20

203,0

cr

crcrk

TkClLog

Figure 2.7- Critical chlorides threshold dependence of temperature and effect of crevice

(dashed lines).

2.4.3 Transitional probability r: meta-passive to passive transition

The probability r is the probability that a stainless steel in a specific environment moves

from the metapassive condition to the absorbing state of passivity. It takes into account the

tendency of the material to repassivate: stainless steels with higher PREN and stronger

passive film have an higher probability of repassivate their metastable pits. Furthermore,

the fluidodynamic condition of the system play an important role: in agitation conditions,

with respect to stagnant, more oxygen, needed for oxide layer repassivation, arrive to the

metal surface by diffusion or convection and chloride ions can be moved away from the

pit; the high velocity of the electrolyte results in washout of the aggressive pit chemistry

(acidic solution by hydrolysis of metal ions), making pit propagation more difficult.

It should be pointed out that, even if r =1, there is always a probability of pitting different

from 0 if the material is not under adequate cathodic protection (p < 1).

Markov model: state of art Chapter 2

39

The expression of r (Eq. 2.23) is derived from the known trend of R: the repassivation

probability increases slowly with fluid velocity until 0,5 m/s, at 1-1,5 m/s increases

dramatically, then stabilizes and for velocity higher than 25 m/s erosion corrosion can

occur [16].

Eq. 2.23 4

min 2,0exp11 vrr

Where v is the fluid velocity and rmin (eq. 2.24) is a parameter which depends on the

stainless steel composition.

Eq. 2.24

2,3

min50

PRENr

High PREN stainless steel are more able to repassivate than low PREN metals. In stagnant

condition this difference is large but increasing fluid velocity it vanishes (Fig. 2.8) because

of the large oxygen supply. This consideration is taken into account imposing rmin equal to

zero for PREN higher than 49: fluid velocity does not affect the pitting corrosion behavior

of high PREN stainless steels and r, then, becomes equal to one (Eq. 2.23).

Figure 2.8- Velocity dependence of r probability.

Markov model: state of art Chapter 2

40

2.4.4 Transitional probability p: meta-pitting to pitting transition

The p-probability is the probability that a stainless steel in a specific environment moves

from the metapitting condition to the pitting absorbing state. If the metal is in cathodic

protection (if the potential E of the material in a specific environment is lower than the

protection potential Eprot) p is zero because corrosion is not thermodynamically possible.

It follows that:

Eq. 2.25

Figure 2.9 shows the potential dependence of p-probability for different stainless steels: for

example, at potential of 400 mV SCE p-probability of AISI 304 stainless steel is 70%

which decreases to 20% considering a PREN 40 duplex stainless steel.

Figure 2.9- Potential dependence of p probability.

Markov model: state of art Chapter 2

41

The protection potential is considered independent from chlorides concentration (this could

be too restrictive) and a linear dependence from PREN is assumed (Fig. 2.10):

Eq. 2.26 50

760,0PREN

E prot

The potential is expressed in Volt vs SCE and 0,760 V SCE is the protection potential of

carbon steel, considered as a zero PREN stainless steel.

Figure 2.10- PREN dependence of protection potential.

2.4.5 Example of R calculation

In the following tables are reported the results (expressed by R and transitional

probabilities) obtained from the MATLAB® implementation of the five-steps Markov

model with different input data in terms of temperature, chlorides concentration, pH and

fluid velocity. Two materials are considered: AISI 304 (PREN 18) and AISI 316 (PREN

24); the free corrosion potential is set equal to 0 V SCE for stainless steel AISI 304, and

equal to 0,100 V SCE for AISI 316. Figure 2.11 shows the MATLAB®

window with

transitional probabilities, transition matrix and transition vector after input data

Markov model: state of art Chapter 2

42

implementation: as example AISI 304 stainless steel at pH 7, 20°C , fluid velocity of 0,5

m/s and default corrosion potential is considered.

The results are plausible on the basis of plant experiences and empirical considerations

[17]. From this recognition the need of laboratory tests aimed to validate the model.

Figure 2.11- Matlab implementation of the Markov model.

Markov model: state of art Chapter 2

43

Table 2.1- AISI 304, pH= 7, E= 0 V SCE

[Cl] ppm V (m/s) r p 20°C 30°C 50°C

m R m R m R

10

0

0,5

2

0,04

0,05

0,96

0,23

1

1

1

1

1

1

1

1

0,63

0,25

0,29

0,88

200

0

0,5

2

0,75

0,42

0,48

0,94

0,39

0,11

0,14

0,73

0,05

0,01

0,01

0,18

500

0

0,5

2

0,47

0,14

0,18

0,79

0,18

0,04

0,05

0,48

0,02

0

0

0,8

Table 2.2- AISI 304, E= 0 V SCE, v= 1,5 m/s, T=20 °C

pH r p 50 ppm 200 ppm 1000 ppm 5000 ppm

m R m R m R m R

3

5

7

8

10

12,6

0,65 0,22

0,35

0,80

1

1

1

1

0,62

0,93

1

1

1

1

0,10

0,33

0,78

0,95

1

1

0,26

0,60

0,91

0,98

1

1

0,02

0,08

0,26

0,44

0,88

1

0,06

0,20

0,52

0,71

0,96

1

0,01

0,02

0,06

0,11

0,36

0,91

0,01

0,05

0,16

0,27

0,72

0,97

Table 2.3- AISI 316, pH=7, E= 0,100 V SCE

[Cl] ppm V (m/s) r p 20°C 30°C 50°C

m R m R m R

200

0

0,5

2

0,11

0,12

0,96

0,21

1

1

1

1

0,89

0,81

0,82

0,97

0,20

0,11

0,12

0,53

1000

0

0,5

2

0,75

0,61

0,63

0,93

0,36

0,22

0,24

0,72

0,04

0,02

0,03

0,17

5000

0

0,5

2

0,24

0,14

0,16

0,60

0,08

0,05

0,05

0,30

0,01

0

0

0,04

Markov model: state of art Chapter 2

44

Table 2.4- AISI 316, E= 0,100 V SCE, v=1,5 m/s, T=20°C

pH R p 200 ppm 1000 ppm 5000 ppm 25000 ppm

m R m R m R m R

3

5

7

8

10

12,6

0,68 0,21

0,39

0,84

1

1

1

1

0,68

0,95

1

1

1

1

0,10

0,31

0,75

0,93

1

1

0,26

0,60

0,91

0,98

1

1

0,02

0,07

0,24

0,41

0,86

1

0,06

0,20

0,51

0,70

0,95

1

0,01

0,02

0,05

0,10

0,33

0,89

0,01

0,05

0,16

0,27

0,62

0,96

2.4 STATISTICAL EVALUATION OF CORROSION DATA

As already discussed in section 2.1, pitting corrosion phenomena are intrinsically

stochastic and, in order to describe them, a statistical approach is mandatory. Follows a

summary of the basics of statistical evaluation of corrosion data aimed to the description of

the propagation stage of pitting corrosion.

The use of probability concepts in describing the corrosion phenomena was first introduced

by Evans, Mears, and Queneua in 1933: they designed an experiment for demonstrating the

concept of corrosion probability [33]. As illustrated in Figure 2.12, wax lines were drawn

on the surface of an iron plate, dividing the surface area in N sections, which were then

covered with a thin film of water. This procedure was equivalent to preparing N separated

specimens exposed to an identical corrosion condition. After exposure for a fixed time

under a mixed gas atmosphere consisting of oxygen and nitrogen, n squares were corroded.

The corrosion probability was calculated as:

Eq. 2.12 N

nP

The sample survival probability is, then, calculated as:

Eq. 2.13 N

nPs 1

Markov model: state of art Chapter 2

45

The pitting probability test can be conducted to determine the susceptibility of metals to

pitting, but it will not provide information about the rate of propagation, and the results are

only applicable to the exposure conditions [22].

Figure 2.12- Demonstration of the concept of corrosion probability by Mears and Evans

[33].

2.4.1 Corrosion data distributions

The distribution of corrosion data can be reduced to several basic probability distributions,

listed in Table 2.5.

Table 2.5- Examples of probability distribution in corrosion [33].

Probability distribution Examples in corrosion

Normal distribution Pitting potential

Log-Normal distribution SSC-failure time

Exponential distribution Induction time for pit generation

SCC and hydrogen embrittlement failure time

Extreme value distribution

Gumbel distribution

Weibull distribution

Maximum pit depth

SCC failure time

Generalized extreme values distribution Maximum pit depth

Fatigue crack depth

Markov model: state of art Chapter 2

46

The various breakdown potentials obtained for the same material from different identical

tests are not considered as univocal but as distributed potentials [20]. All distributions obey

the normal (Gaussian) distribution [18, 20, 33].

Figure 2.13- Normal (Gaussian) distribution [23].

The normal distribution is a bell shaped curve (Fig. 2.13) which fits the histogram of most

corrosion data [33]. The curve is described by the probability density function, f(x):

Eq. 2.14

2

2

2exp

2

1

xxf

Where µ and σ are the mean and standard deviation, respectively, which determine the

shape of the curve. The area under the curve gives the probability of occurrence, calculated

by the cumulative probability function, F(x):

Eq. 2.15

dx

xdxxfxF

2

2

2exp

2

1)(

Each set of [x, F(x)], for the pitting potential and the corresponding cumulative probability,

can be plotted on normal probability paper. The straight line fitting the points, shown in

Figure 2.14, indicates that the measured data obey the normal probability distribution [18,

33].

Markov model: state of art Chapter 2

47

Figure 2.14- Probability plot for the distribution of pitting potential on normal probability

paper [33].

The Poisson distribution is used to describe random phenomena observed in rare events

[33]. Pits generation is a good example of a random process that can be described using the

Poisson distribution [18, 27, 33], expressed as:

Eq. 2.16 mx

mxP

x

exp

!

Where P(x) is the probability of occurrence of x pits in unit area and m is the mean or

expected value of x. Figure 2.15 shows distribution curves of pits obeying the Poisson

distribution.

Figure 2.15- Distribution curves of pits obeying the Poisson distribution. [33]

Markov model: state of art Chapter 2

48

2.4.2 Extreme value statistics

When the required corrosion data are not available, corrosion engineers design a laboratory

test that simulates field operating conditions. In some cases, they may also be asked to

predict the remaining life of apparatus in operation. The size of the coupon and the

duration of testing may change over a wide range depending on the purpose of the test and

the requirements of the client. In the laboratory test, coupons of relatively small area (e.g. 1

cm2) are used and tested in a relatively short time (hours, days or weeks depending on the

test type) under accelerating conditions, whereas larger coupon, several times 10 cm2, are

required in pilot plant tests that typically last for at least a few months [33]. Difference in

size as well as in duration between the laboratory test and the field examination are

extremely large; a method for bridging these large differences is provided by the statistical

theory of extreme values [18, 33]. The extreme value distribution can be reduced to three

types of asymptotic distributions for an infinite number of samples, and which of the three

types applies in a given situation depends on the initial distribution:

Eq. 2.17 (-x) exp-exp~xF Type I, Gumbel distribution

Eq. 2.18 kxF

x- exp~ Type II, Caucy distribution

Eq. 2.19 kxF x-w- exp~ Type III, Weibull distribution

When corrosion data for the maximum and the minimum value are collected, one must

decide which type of extreme value distribution should be fitted the observed data.

The Gumbel distribution is used to analyze pit depth distribution. It is not the overall

corrosion rate or the number of pits that are of interest, but the deepest pits because they

cause the failure of the system [21].

In order to estimate the maximum depth of pits over the larger surface area from which

specimens of small area are extracted, the Gumbel distribution is expressed as [33]:

Markov model: state of art Chapter 2

49

Eq. 2.20

-x -exp- expxF

Where F(x) is the cumulative probability of pit depth, x, and λ and α are the location and

scale parameters, respectively. The probability density function, f(x) is given by:

Eq. 2.21

xxxf exp exp

1

The maximum pit depth is obtained from experimental results and tabulated. An example

of plotting the pit depth data is shown in Figure 2.16 [20]. The Gumbel probability is

constructed with values of y scaled on the vertical axis and the associated cumulative

probabilities (Eq. 2.22).

The reduced variable y is defined as:

Eq. 2.22

xy

Then,

Eq. 2.23 yFy lnln

Eq. 2.24 N

iyF

11

Where i is the ith

position of the ordered values of x, in descending order, and N is the total

number of samples. Plotting y as a function of x (Fig.2.16) yields a straight line, and its

slope is 1/α, and the intercept at y=0 gives λ.

Markov model: state of art Chapter 2

50

Figure 2.16- Probability plot of the distribution of pit depth in samples of small area on

Gumbel probability paper, from which the maximum pit depth for the larger surface area

can be extimated [33].

The third type of extreme value distribution for the minimum value, the Weibull

distribution, is used often in reliability engineering to analyze failure life distribution in

stress corrosion cracking situations [18, 33]:

Eq. 2.25

m

ttF

exp1

Where γ, η and m are the location, scale and shape parameters, respectively.

The shape parameter is an important parameter because it controls the shape of the

probability density function f(t), and also the failure time λ(t):

Eq. 2.26

m

mm ttm

dt

tdFtf

exp

)( 1

Eq. 2.27

1

1

mmtm

tF

tft

Markov model: state of art Chapter 2

51

Without going deeper into this topic, some graphs are reported [33] which show

probability plots of the SCC failure time on Weibull probability paper (Fig. 2.17, 2.18).

Figure 2.17- Probability plots on Weibull probability paper of the SCC failure time of

austenitic stainless steel in boiling MgCl2 solution [33].

Figure 2.18- Weibull probability plots of the SCC failure time of high strength steel bolts

exposed under various environmental conditions. [33]

Markov model: state of art Chapter 2

52

The extreme value statistical theory is a powerful tool to analyze localized corrosion

quantitatively but limited in analysis of the time-dependent probabilistic aspects of pitting

corrosion, which would be very useful in assessing the reliability of a corroding system

[18, 25]. Since the initiation time prediction plays a critical role for engineering

application, the attention has been focused on the experimental validation of the five-steps

Markov model.

Validation of the proposed Markov model: potentiostatic polarization test Chapter 3

53

Chapter 3

VALIDATION OF THE PROPOSED MARKOV MODEL:

POTENTIOSTATIC POLARIZATION TEST

3.1 AIM OF THE TEST

The results obtained from MATLAB® implementation of the five steps Markov model,

which are summarized in tables of section 2.4.5, are considered reasonable on the basis of

engineering knowledge of stainless steels behavior [16, 17]. Despite that, they require the

design and set up of experimental tests aimed to their validation.

The first step of the Markov model validation work has implied the run of potentiostatic

polarization tests on stainless steels with different PREN, progressive increasing the

content of chlorides in solution at pH 7 obtained with distilled water and addition of

sodium chloride (NaCl). Table 3.1 reported the chemical composition of the test materials.

Table 3.1- Chemical composition of the test materials.

AISI

grade

EN

grade PREN C % Mn % P % S % Si % Cr % Ni %

430 1.4016 17 0,08 1 0,04 0,015 1 17 -

304 4.4301 18 0,07 2 0,045 0,015 1 18 9

470LI 1.4613 24 0,03 1 - 0,015 1 24 -

3.2 POTENTIOSTATIC POLARIZATION TEST

Potentiostatic and potentiodynamic polarization tests are electrochemical techniques

commonly used for corrosion testing. Electrochemical tests require an electrochemical cell

(Fig. 3.1) which includes, in addition to the metal to study (working electrode, W), a

counter electrode (CE), a reference electrode (EF) and a source of electric work: the

reference electrode has a well known standard potential and is used to measure the

potential of the working electrode (the sample); the counter electrode is used to make a

connection with the electrolyte so that the current can be applied to the working electrode;

Validation of the proposed Markov model: potentiostatic polarization test Chapter 3

54

the source of electric work is, in the case of potentiostatic tests, the potentiostat, an

instrument that applies a current to the specimens which enables the potential to be

controlled in a desired way.

Figure 3.1- Schematic representation of an experimental set up [4].

Each test material was polarized through the potentiostat to +50 mV and +150 mV with

respect to the free corrosion potential. For each polarization potential the chlorides

concentration is varied from 100 to 1000 mg/L. For each chlorides content (100, 300 and

1000 mg/L), the number of corroded sample is registered after a week.

The tests is carried out at two different temperatures, 25° C and 40° C, in stagnant

conditions.

3.3 EXPERIMENTAL SET UP

3.3.1 Samples preparation

For each material, samples of size 3 x 3 cm (Fig. 3.2) were cut from provided sheets of

dimensions 18 x 27 x 0.1 cm. They are electrically connected to an insulated copper cable

by spot welding of the back surface (Fig. 3.3).

The final surface to be exposed to the solution was 2 x 2 cm: the back surface and lateral

edges of the sample were coated with an insulating polymer resin with high covering

power (Fig. 3.4). A commercial product consisting of a bi-component epoxy resin with

thixotropic properties was used, which guarantees high coverage of the surface also in

Validation of the proposed Markov model: potentiostatic polarization test Chapter 3

55

correspondence of angular points of the plate, as the edges. As the final surface exposed to

the test solution should not undergoing any treatment which would affect its roughness

(must not be blasted or mechanically abraded), it was only cleaned with acetone.

Figure 3.2- Stainless steel sample 3x3

cm.

Figure 3.3- Welded cable on the sample back

surface.

Figure 3.4- Coated back surface. Figure 3.5- Exposed surface (2x2 cm).

Validation of the proposed Markov model: potentiostatic polarization test Chapter 3

56

3.3.2 Electrochemical cells assembly

In order to ensure that the ratio between the test solution volume and the sample surface is

at least 0,2 mL/mm2, according to the standard which rules corrosion immersion tests [34],

20 L of solution are placed into tanks of dimensions 40 x 40 x 20 cm and capacity 30 L.

The test cell consist of 20 stainless steel samples electrically connected, a Ti-MMO counter

electrode and a SSCsat reference electrode (silver-silver chloride in KCl saturated solution,

+0,200 V SHE), which is placed in the tank equidistant from all the samples. Figure 3.6

shows a scheme of the test cells. For each material, twenty samples were positioned in the

tank along a circle drawn on tank cover so as to ensure homogeneous distribution of

current (Fig. 3.7 and 3.8). They were short-circuited and connected to the Working (W) of

the potentiostat. Each sample is series connected to an electrical resistance of 10 kΩ which

is required for voltage measurement, in order to calculate the circulating current. Also

counter electrode and reference electrode are connected to the potentiostat (Fig. 3.9).

Figure 3.6- Scheme of the test cell and electrical connections.

Validation of the proposed Markov model: potentiostatic polarization test Chapter 3

57

Figure 3.7- Cell cover with holes.

Figure 3.8- Reference electrode, counter electrode and samples in the test cell.

Fig. 3.9- Electrical connection of the electrochemical cells to the potentiostat.

Validation of the proposed Markov model: potentiostatic polarization test Chapter 3

58

3.3.3 Experimental procedure

The first week three tanks (one for each material) were filled with a room temperature test

solution: in order to obtain an initial solution of 100 mg/L Cl-, 0,17 g/L NaCl were added

to 20 L of distilled water. Samples were kept 24 h in free corrosion condition until steady

state potential was measured (Ecorr). They were anodically polarized at E1= + 50 mV vs

Ecorr, as summarized in Table 3.1. The value of the ohmic drop on the shunts was

monitored daily (Fig. 3.9) and registered on an Excel Word file:

if this value was zero, the specimen was still in passive condition.

if the value was greater than 5 mV, the sample was considered in corrosion

condition.

if the measure of the ohmic drop was exceeding 5 mV for two consecutive days, the

sample was detatched from the test circuit.

An ohmic drop of 5 mV corresponds to a circulating current density of 1,25 mA/m2, as

shown in Equation 3.1.

Eq. 3.1 2244 m

mA25,1

m10410

V005,0

SR

V

S

Ii

Where V is the voltage measured across the resistor (V), R is the resistance value (Ω) and

S is the sample surface (4 cm2). The value 5 mV has been chosen on the basis of corrosion

test experience: when corrosion starts the measured ohmic drop is immediately of the order

of 200 mV and for conservative reasons the upper limit of passivity condition is chosen to

be that corresponding to an ohmic drop of 5 mV.

Validation of the proposed Markov model: potentiostatic polarization test Chapter 3

59

Figure 3.10- Ohmic drop on the resistance measurement.

At the end of the week the percentage of corroded samples was calculated and they were

replaced with new specimens. Still passive samples were not replaced: this experiment is

based on the assumption that pitting corrosion is a Markov process and, therefore, samples

have no memory of their past history. The chlorides content was increased to 300 mg/L,

adding 0,33 g/L NaCl to the solution and keeping the temperature constant.

The ohmic drops value on the shunt was monitored daily for a week and corroding samples

were detatched as previously described. At the end of the week the corroded samples were

replaced with new specimens. The chlorides content was increased to 1000 mg/L, adding

1,16 g/L NaCl to the solution and keeping the temperature constant.

The monitoring and the detachment procedure occured in the same way also during the

third week.

Table 3.2- Experimental condition, 20°C, E1

Material Temperature Chlorides (mg/L) Ecorr (V SSC) E1 (V SSC)

AISI 430 25 100, 300, 1000 -0,110 -0,060

AISI 304 25 100, 300, 1000 0,050 0,100

470LI 25 100, 300, 1000 -0,100 -0,050

Validation of the proposed Markov model: potentiostatic polarization test Chapter 3

60

The potentiostatic test at polarization potential E2= +0,150 V vs Ecorr have been carried out

with the same procedure described above and summarized in Table 3.3.

Table 3.3- Experimental conditions 20°C, E2

Material Temperature Chlorides (mg/L) Ecorr (V SSC) E2 (V SSC)

AISI 430 25 100, 300, 1000 0,050 0,200

AISI 304 25 100, 300, 1000 0,060 0,210

470 LI 25 100, 300, 1000 0,050 0,200

Similarly, also 40°C tests start: three tanks are assembled as described in section 3.2.2 and

with the aid of a thermostat, the temperature of a 100 mg/L Cl- solution is raised to 40 °C.

The samples are left 24 h in free corrosion and the open circuit potential is measured and

registered. The specimens are polarized to E1= +50 mV vs Ecorr (Table 3.4), the ohmic

drops across the resistors are monitored daily and corroding samples detached from the

circuit. After a week corroded samples are replaced and the chlorides concentration is

increased to 300 mg/L. Likewise, the following week the chlorides content is raised 1000

mg/L. Each week the corroded specimens percentage is calculated. Table 3.4 summarizes

the experimental conditions.

Table 3.4- Experimental conditions 40°C, E1

Material Temperature Chlorides (mg/L) Ecorr (V SSC) E1 (V SSC)

AISI 430 40 100, 300, 1000 -0,020 0,030

AISI 304 40 100, 300, 1000 -0,020 0,030

470 LI 40 100, 300, 1000 0,000 0,050

The same experimental set up and monitoring is carried out for three weeks at 40 °C

polarized to E2*= +300 mV vs Ecorr, as summarized in Table 3.5.

Table 3.5- Experimental conditions 40°C, E2*

Material Temperature Chlorides (mg/L) Ecorr ( V SSC) E2* (V SSC)

AISI 430 40 100, 300, 1000 0,025 0,325

AISI 304 40 100, 300, 1000 0,000 0,300

470 LI 40 100, 300, 1000 0,000 0,300

Validation of the proposed Markov model: potentiostatic polarization test Chapter 3

61

3.4 RESULTS AND DISCUSSION

Tables 3.5, 3.6 and 3.7 show the results of the potentiostatic polarization tests. For each

experimental condition the percentage of corroded specimens (Eq. 3.2) is computed.

Eq. 3.2 100N

nPc

Where n is the number of corroded samples and N is equal to 20.

Table 3.5- Results of potentiostatic test at E1 and E2 on AISI 430 at 25 and 40°C

Material T (°C) Polarization level vs

Ecorr E (V SSC)

Chlorides (mg/L)

100 300 1000

Week 1 Week 2 Week 3

AISI 430

25 +50 mV -0,060 0% 0% 0%

+150 mV 0,200 10% 5% 60%

40 +50 mV 0,030 0% 0% 0%

+300 mV 0,325 95% 100% 100%

Table 3.6- Results of potentiostatic test at E1 and E2 on AISI 304 at 25 and 40°C

Material T (°C) Polarization level vs

Ecorr E (V SSC)

Chlorides (mg/L)

100 300 1000

Week 1 Week 2 Week 3

AISI 304

25 +50 mV 0,100 0% 0% 0%

+150 mV 0,210 15% 0% 10%

40 +50 mV 0,030 0% 0% 0%

+300 mV 0,300 10% 0% 25%

Table 3.7- Results of potentiostatic test at E1 and E2 on 470LI stainless steel at 25 and 40°C

Material T (°C) Polarization level vs

Ecorr E (V SSC)

Chlorides (mg/L)

100 300 1000

Week 1 Week 2 Week 3

470LI

25 +50 mV -0,050 0% 0% 0%

+150 mV 0,200 5% 5% 15%

40 +50 mV 0,050 0% 0% 0%

+300 mV 0,300 5% 0% 10%

Validation of the proposed Markov model: potentiostatic polarization test Chapter 3

62

The results obtained from the laboratory tests are compared from those arising from

MATLAB® implementation of the five-steps Markov model. The comparison is shown in

Tables 3.8, 3.9 and 3.10 and in the corresponding histograms; Tables also show the

transitional probabilities dependence on the input parameters.

It’s clear that a large discrepancy exists between experimental and Markov model results;

anyway, this gap seems to decrease as the testing condition becomes more aggressive

(higher potential, higher temperature and chlorides concentration), expecially for AISI 430

stainless steel. This will be the starting observation for the model revision of the following

chapters. Before that, some consideration should be done on both, experimental set up and

Markov model state of art: corrosion data obtained by laboratory tests question the

common engineering knowledge of stainless steels corrosion behavior; on the other hand

the results of this five-steps Markov model can lead to too conservative materials selection

criteria. Test design and experimental procedure have been carried out properly, but also

corrosion data must be interpreted carefully: for example, environmental conditions, as

potential, solution temperature, pH and chemistry, are homogeneous in space and

controlled in time during laboratory tests; this does not occur in field conditions, where

temperature and aggressive species concentration vary in time and are not homogeneous all

over the metal surface, biofilm and pollutant are present, exposed surfaces are larger and

contain higher density of pitting initiation sites. Furthermore, in real cases, to which

Markov model applies, materials lie in corrosive environment for years while this

potentiostatic tests last three weeks. As underlined in [2], corrosion laboratory tests are

frequently the best available source of data for materials selection: since most equipment is

intended to perform for many years, whereas the time available for prior testing is short,

accelerating test are often necessary; if the acceleration (higher temperature, higher stress,

lower pH, higher chlorides concentration, or, as in this case, application of an anodic

polarization potential) produce the same mode of failure that is expected under non-

accelerated nominal and longer term conditions, results from such testing provide

credibility to prediction. Despite the commonly agreed reliability of accelerated corrosion

test results, one can doubt on the choice of this potentiostatic test duration asking if a week

is sufficient for pit initiation. Corrosion engineers experience suggest that pits start in a few

days after immersion in aggressive solution and practical consideration have lead to the

previously described experimental design.

Validation of the proposed Markov model: potentiostatic polarization test Chapter 3

63

The equations of transitional probabilities of Markov model, described in Chapter 2, are

empirical and based on engineering knowledge of corrosion behavior of stainless steels.

An attempt to justify and modify these equations through literature data elaboration and

laboratory tests is made in the following chapters.

Table 3.8- AISI 430 (PREN 17) experimental corrosion probability and Markov probabilities.

T (°C) pH Cl (mg/L) E (V SCE) Pc

EXP

1-R

Markov R p m

20 7

100

-0,001

0% 42% 0,0317 0,1776 0,8856

300 0% 84% 0,0317 0,1776 0,5145

1000 0% 96% 0,0317 0,1776 0,1949

100

-0,156

10% 64% 0,0317 0,4372 0,8856

300 5% 93% 0,0317 0,4372 0,5145

1000 60% 98% 0,0317 0,4372 0,1949

40 7

100

-0,014

0% 97% 0,0317 0,2587 0,1949

300 0% 99% 0,0317 0,2587 0,0697

1000 0% 100% 0,0317 0,2587 0,0214

100

0,281

95% 99% 0,0317 0,5869 0,1949

300 100% 100% 0,0317 0,5869 0,0697

1000 100% 100% 0,0317 0,5869 0,0214

Validation of the proposed Markov model: potentiostatic polarization test Chapter 3

64

Plot 3.1- Experimental and theoretical corrosion probability comparison for AISI 430 at

20°C.

Plot 3.2- Experimental and theoretical corrosion probability comparison for AISI 430 at

40°C.

Validation of the proposed Markov model: potentiostatic polarization test Chapter 3

65

Table 3.9- AISI 304 (PREN 18) experimental corrosion probability and Markov probabilities.

T (°C) pH Cl (mg/L) E (V SCE) Pc

EXP

1-R

Markov r p m

20 7

100

0,056

0% 34% 0,0318 0,3079 0,9392

300 0% 84% 0,0318 0,3079 0,6068

1000 0% 96% 0,0318 0,3079 0,2442

100

0,166

15% 42% 0,0318 0,4258 0,9392

300 0% 88% 0,0318 0,4258 0,6068

1000 10% 97% 0,0318 0,4258 0,2442

40 7

100

-0,014

0% 95% 0,038 0,2398 0,2442

300 0% 98% 0,038 0,2398 0,0891

1000 0% 100% 0,038 0,2398 0,0276

100

0,256

15% 98% 0,038 0,5313 0,2442

300 0% 99% 0,038 0,5313 0,0891

1000 25% 100% 0,038 0,5313 0,0276

Plot 3.3- Experimental and theoretical corrosion probability comparison for AISI 304 at

20°C.

Validation of the proposed Markov model: potentiostatic polarization test Chapter 3

66

Plot 3.4- Experimental and theoretical corrosion probability comparison for AISI 304 at

40°C.

Table 3.10- 470 LI (PREN 24) experimental corrosion probability and Markov probabilities.

T (°C) pH Cl (mg/L) E (V SCE) Pc

EXP

1-R

Markov r p m

20 7

100

-0,094

0% 0% 0,0955 0,0802 1

300 0% 1% 0,0955 0,0802 0,9869

1000 0% 24% 0,0955 0,0802 0,7274

100

0,156

5% 0% 0,0955 0,2879 1

300 5% 4% 0,0955 0,2879 0,9869

1000 15% 96% 0,0955 0,2879 0,7274

40 7

100

0,006

0% 38% 0,0955 0,1529 0,7274

300 0% 75% 0,0955 0,1529 0,3516

1000 0% 92% 0,0955 0,1529 0,1219

100

0,246

5% 60% 0,0955 0,3815 0,7274

300 0% 88% 0,0955 0,3815 0,3516

1000 10% 97% 0,0955 0,3815 0,1219

Validation of the proposed Markov model: potentiostatic polarization test Chapter 3

67

Plot 3.5- Experimental and theoretical corrosion probability comparison for 470 LI at

20°C.

Plot 3.6- Experimental and theoretical corrosion probability comparison for 470 LI at

40°C.

p-probability: a review of the meta-pitting to pitting transition Chapter 4

68

Chapter 4

p-PROBABILITY:

A REVIEW OF THE META-PITTING TO PITTING TRANSITION

4.1 INTRODUCTION

The transitional probability p is the probability that the system moves from the metapitting

state to the pitting absorbing state. If p-probability is zero, pitting corrosion would not

occur: the only condition that allows this to happen with certainty is the cathodic

protection. Therefore, p is chosen to be dependent on the difference between the potential

of the metal in a specific environment and the protection potential, defined as the

repassivation potential. The protection potential is assumed to be linearly dependent on the

PREN but independent on the chloride concentration of the solution. The p-probability

equations and the p-probability-potential trend (Fig. 4.1), already discussed in section

2.4.4, are reported below:

Eq. 4.1

Eq. 4.2 50

PREN760,0Eprot

p-probability: a review of the meta-pitting to pitting transition Chapter 4

69

Figure 4.1- Potential dependence of p probability.

As widely discussed, Markov model equations were proposed on the basis of the

engineering knowledge in the field of materials selection, where localized corrosion

represents a risk for materials service life. In this work a bibliographic research and

experimental tests were carried out in order to confirm (or modify) the equations initially

proposed. The compare between experimental and theoretical corrosion probability,

proposed in section 3.4, suggests that, since, the gap between the results diminishes

increasing the potential, the first consideration should be done about the shape of the p-

probability curve: for low potential p-probability should be lower than that predicted by the

existing Markov model. Furthermore, an asymptotic behavior should be taken into

account: it’s reasonable to think that pitting probability does not increase indefinitely with

potential but tends to one asymptotically; indeed, the p-probability expression for potential

higher than protection potential should be modified. On the contrary, the condition p= 0 if

E ≤ Eprot should be not changed because set its basis on thermodynamic reasoning (section

2.4.4).

Moreover, the Eprot-PREN relation (Eq. 4.2) must be checked with literature data and

experimental results. For sake of simplicity, the linear dependence will be considered still

valid; considering carbon steel protection potential as that corresponding to a zero PREN

stainless steel is a reasonable and useful starting point.

p-probability: a review of the meta-pitting to pitting transition Chapter 4

70

4.2 STATISTICAL ELABORATION OF LITERATURE DATA

4.2.1 Pitting potential distribution

A significant amount of literature data is available on pitting potential of various stainless

steels in environment with different chlorides concentration. Otherwise, there is a lack of

data on protection potential values. For these reasons, p-equations rework starts from

pitting potential data collection. Pitting potential values for different materials are

extrapolated from tables and graphs of books [1, 2, 11] and articles [13, 15, 35, 36] and

tabulated. Chlorides concentration solution above 10 g/L, room temperature and neutral pH

conditions are taken into account (Appendix A). The attention, then, has been focused on

graph of Figure 4.2, which shows pitting potential trend varying with chromium content,

main element which defines PREN (Eq.1.1). Plot 4.1 shows an acceptable match between

selected data and trend derived from Figure 4.2; furthermore, it shows the scattering of

pitting potential values: the probabilistic approach is, then, mandatory.

Figure 4.2- Effect of chromium content on pitting potential of iron-chromium alloys [2].

p-probability: a review of the meta-pitting to pitting transition Chapter 4

71

Plot 4.1- Selected data are reported on a potential-PREN graph, compared with curve of Figure

4.2 and values scattering is underlined.

As shown in Figure 4.2 (red circle), pitting potential does not vary dramatically for

stainless steels with PREN between 17 and 20, hence, only data concerning these materials

are selected and elaborated. From this point forward no more restriction on chlorides

content are made but, again, only room temperature and neutral pH conditions are

considered (Appendix A, bold highlighted values).

Pitting potential obey Gaussian distribution (section 2.5.1); accordingly, normal and

cumulative probability functions are calculated for the selected data, known the mean and

the standard deviation (Eq. 2.14 and 2.15): the curves are reported in Plot 4.2 and 4.3 and

the values in Appendix B. The pitting potential for PREN 17 stainless steel has been

chosen as that corresponding to P= 0,10: the probability that pitting occurs for lower

potential is 10% (Plot 4.2).

p-probability: a review of the meta-pitting to pitting transition Chapter 4

72

Plot 4.2- Cumulative probability function curve

and definition of pitting potential.

Plot 4.3- Normal distribution function curve of

pitting potential.

4.2.2 Protection potential determination

The assumptions of linear dependence of protection potential with PREN and of

independence on chlorides concentration are considered still valid. Chlorides independence

may be a strong assumption but the whole model, in which each transitional probability is

affected by different parameters, must be considered: the real system is described by the

transition matrix and the distribution vectors (section 2.2), which interconnect transitional

probabilities and their influence factors.

Considering engineering experience on corrosion and cathodic protection [4], it is assumed

that the protection potential value is 300 mV lower than the pitting potential. Plot 4.4

shows this consideration applied to the theoretical curve, derived from Fig. 4.2.

p-probability: a review of the meta-pitting to pitting transition Chapter 4

73

Plot 4.4- Protection potential determination.

Then, for PREN 17 stainless steels the protection potential is:

Eq. 4.3

Since carbon steel (which is considered a 0 PREN stainless steel) protection potential is -

0,760 V SCE and PREN 17 protection potential is -0,342 V SCE (Eq. 4.3), the slope of the

straight line Eprot-PREN would be 40

1.

Eq. 4.4 40

PREN760,0Eprot

Plot 4.5 shows the old-Markov model and the new-Markov model straight lines compared

with the “literature” curve, obtained from Plot 4.4: a good match is observed between the

reviewed trend and the theoretical curve.

p-probability: a review of the meta-pitting to pitting transition Chapter 4

74

Plot 4.5- Eprot-PREN trend.

4.2.3 Calculation of p-probability

As widely discussed, p-probability depends on the difference between the potential

assumed by the material in a specific environment and the protection potential. The idea is

to modify the shape of the p-probability curve (Eq. 4.5), taking into account an asymptotic

behavior and the prediction of lower probability for low potential (section 4.1).

Eq. 4.5

The cumulative probability function of the pitting potential distribution, which gives the

probability of occurrence, is used as model curve: for each probability value, Epitt is

substituted with E-Eprot, where Eprot is the mean value between the new Markov model

protection potential of stainless steels with PREN from 17 to 20 (Appendix B). A and B

constant (Eq 4.5) are calculated as the parameters which minimize the difference between

p-probability: a review of the meta-pitting to pitting transition Chapter 4

75

the cumulative distribution and the p-probability curve. The resulting values are A= 2

3and

B= 3:

Eq. 4.6 3

protEE2

3exp1p

Plot 4.6 shows the “old” Markov model p-probability curve (dashed line) and the reviewed

one, which satisfies the requirement of asymptotic behavior and prediction of lower

probabilities for low potential.

Plot 4.6- p probability- (E- Eprot) trend.

Finally, p-probability-potential curves for different stainless steels are shown in Plot 4.7: a

first improvement in the equation revision has been made: the new curves are shifted on

the right with respect the old curves, then predicting lower probabilities; for example, at

potential of 100 mV SCE, p-probability for AISI 304 for the “old” model was 35% while

decreases to 20% for the reviewed model.

p-probability: a review of the meta-pitting to pitting transition Chapter 4

76

Plot 4.7- p probability-potential trend for different stainless steels: comparison between new and

old Markov model.

4.3 CYCLIC POTENTIODYNAMIC POLARIZATION TESTS

p-probability equations (Eq. 4.4 and 4.5) were obtained through literature data elaboration;

with the aim of confirm them, laboratory tests were carried out in order to obtain, in

specific experimental condition, pitting and protection potential.

The relative susceptibility to localized corrosion for iron-, nickel-, or cobalt-based alloys is

usually determined through cyclic potentiodynamic polarization measurements. ASTM

G61 [40] covers the procedure for conducting them and the experimental procedure which

can be used to check experimental techniques and instrumentation.

p-probability: a review of the meta-pitting to pitting transition Chapter 4

77

The voltage applied between the working electrode and the inert counter electrode is

ramped at a continuous slow rate (0,6 V/h) relative to a reference electrode using a

potentiostat. The voltage is first increased in the anodic direction (forward scan); then, the

voltage scan direction is reversed at some chosen current or voltage (ASTM G61 suggests

when current reaches 5 mA). The scan is terminated at another chosen voltage, usually

either the corrosion potential [40] or some potential lower than corrosion potential [2]. The

potential at which the scan is started is the corrosion potential measured when the

corrosion process reaches the steady state; ASTM G61 suggests to start the potential scan

one hour after specimen immersion. The procedure, as outlined in the standards, is not the

only or even necessarily the best way to generate the polarization scan in all situations [1].

Though the generation of the polarization scan is simple, its interpretation can be difficult.

Features identified as important for determining the propensity for localized corrosion are

the protection or repassivating potential and the pitting or breakdown potential (Fig. 4.3).

Figure 4.3- Cyclic polarization curve for a passive metal.

The potential at which the anodic current increases significantly with the applied potential

is the pitting potential. In general, the more noble is the pitting potential, obtained at fixed

scan rate, the less susceptible the alloy is to the initiation of the localized attack.

The second parameter of great interest is the potential at which the hysteresis loop is

completed during reverse polarization scan after localized corrosion propagation. This

potential is taken as the repassivation, Erp, or protection potential, Eprot. In general, once

initiated, localized corrosion can propagate only at potential more positive than the

protection potential [7]; in other words, even after pitting initiation, repassivation will

p-probability: a review of the meta-pitting to pitting transition Chapter 4

78

occur at more negative potential. At potential between Epitt and Eprot, sites that have

initiated can propagate.

Although the cyclic method is a reasonable method for checking relative susceptibility of

alloys to pitting corrosion in different environment, it has been found to have a number of

shortcomings [7]. The major problem concerns the effect of the potential scan rate; the

values of both Epitt and Eprot are strong function of the manner in which the tests are

performed, particularly the potential scan rate used; experimental values of Epitt are linked

to the induction time required for pitting: pitting potential obtained from slow scan rate test

are lower than that from higher scan rate test because the attack has more time to occur and

to propagate. Another complication arises from allowing too much pitting propagation to

occur before reversing the scan direction: the more attack that has been allowed to occur,

the more negative is the Eprot value.

Due to the statistical nature of pitting nucleation, the scatter in the data obtained from

different polarization curves of the same material is expected especially in the forward

scan. The reverse scans are more reproducible, because the local chemistry controls the

repassivation [7].

4.3.1 Experimental set up

Cyclic potentiodynamic polarization tests have been performed on different materials in

order to compare experimental protection potential and new-Markov model protection

potential values. The electrochemical cell scheme is shown in Fig. 4.4: the reference

electrode is SSCsat, the counter electrode Ti-MMC and the working electrode is the test

material sample. Test parameters are reported in Table 4.1.

p-probability: a review of the meta-pitting to pitting transition Chapter 4

79

Fig. 4.4- Electrochemical cell.

Table 4.1- Test parameters.

Exposed surface 0,0001 m2

Chloride concentration 20 g/L

Temperature 20 °C

pH 7

Scan rate 0,166 mV/s

Reversal scan current 3 mA

4.3.2 Results and discussion

4.3.2.1 AISI 430 stainless steel

Several test have been performed on AISI 430 stainless steel and experimental cyclic

potentiodynamic curves are shown in Plot 4.8.

p-probability: a review of the meta-pitting to pitting transition Chapter 4

80

Plot 4.8- Cyclic potentio8ynamic curve for AISI 430 (PREN 17) in 20 g/L NaCl solution.

Plot 4.8 shows that the curves obtained from different tests are similar, which guarantees

the reliability of results, and also shows the expected statistical variability of pitting and

protection potential; furthermore, it’s worth to notice that Eprot are not “passivity”

protection potential, as in Fig. 4.3, but repassivation is achieved for immunity condition. In

Table 4.2 are reported the experimental values of each test and in Table 4.3 are shown

experimental mean values of pitting and protection potential and the comparison with old

(Eq. 4.7) and new (Eq. 4.8) Markov model values (M* notation indicates new Markov

model).

Eq. 4.7 420,050

17760,0MEprot V SCE

Eq. 4.8 335,040

17760,0MEprot

V SCE

Experimental results show a good agreement with the new-Markov model equations: the

discrepancy between Markov model protection potential and experimental values

p-probability: a review of the meta-pitting to pitting transition Chapter 4

81

decreases if equation is modified. Furthermore, the assumption Eprot= Epitt – 300 mV is

justified.

Table 4.2- Experimental values of pitting and protection potential.

Material PREN Test Epitt (V SCE) Eprot (V SCE)

AISI 430 17

1 0,068 -0,252

2 0,160 -0,287

3 0,019 -0,330

4 0,076 -0,321

5 0,117 -0,277

6 -0,077 -0,291

7 0,102 -0,263

Table 4.3- Mean experimental values and Markov model values for AISI 430 stainless steel.

Experimental “Old” Markov model “New” Markov model

Epitt (V SCE) 0,066 - -

Eprot (V SCE) -0,289 -0,420 -0,335

Epitt - Eprot (V) 0,335 0,046 0,131

4.3.2.2 AISI 304 stainless steel

Several test have been performed on AISI 304 stainless steels and cyclic potentiodynamic

curves are shown in Plot 4.9: the consideration done for AISI 304 are still valid.

p-probability: a review of the meta-pitting to pitting transition Chapter 4

82

Plot 4.9- Potentiodynamic curve for AISI 304 in 20 g/L NaCl solution.

Experimental pitting and protection potential are reported in Table 4.4. Markov model

protection potential are obtained from Eq. 4.9 (old-Markov model) and Eq. 4.10 (new-

Markov model) and in Table 4.5 are compared with mean experimental values. Also for

AISI 304 stainless steel the modification of the theoretical equation lead to a better match

with experimental results.

Eq. 4.9 400,050

18760,0MEprot V SCE

Eq. 4.10 310,040

18760,0MEprot

V SCE

p-probability: a review of the meta-pitting to pitting transition Chapter 4

83

Table 4.4- Experimental values of pitting and protection potential.

Material PREN Test Epitt (V SCE) Eprot (V SCE)

AISI 304

18

1 0,385 -0,205

2 0,428 -0,219

3 0,364 -0,204

4 0,434 -0,235

5 0,417 -0,220

Table 4.5- Mean experimental values and Markov model values for AISI 304 stainless steel.

Experimental “Old” Markov model “New” Markov model

Epitt (V SCE) 0,406 - -

Eprot (V SCE) -0,217 -0,400 0,310

Epitt - Eprot (V) 0,622 0,183 0,093

4.3.2.3 AISI 470LI stainless steel

Plot 4.10 shows the cyclic curves obtained from potentiodynamic test carried out on 470 LI

stainless steel. Experimental results are reported in Table 4.6 but they seems not to be

reliable or useful for the compare with Markov model values. This can be explained

considering the fact that these cyclic potentiodynamic curves have features difficult to

interpret: a lot of instability phenomena occur during forward scan, pitting potential seems

to be of the order of oxygen evolution potential and it is not easy to determine where the

hysteresis loop is completed and, then, the protection potential. Further laboratory tests

should be made in order to get reliable values of pitting and protection potentials for high

PREN stainless steels, like cyclic potentiodynamic polarization tests in deareated solutions

or potentiostatic scratch tests [7].

p-probability: a review of the meta-pitting to pitting transition Chapter 4

84

Plot 4.10- Potentiodynamic curve for AISI 470LI in 20 g/L NaCl solution.

Table 4.6- Experimental values of pitting and protection potential.

Material PREN Prova Epitt (V SCE] Eprot (V SCE)

470LI 24

1 0,825 -0,015

2 0,436 -0,329

3 0,945 -0,324

4 0,894 -0,344

5 1,008 -0,322

Min 0,436 -0,344

Max 1,008 -0,015

Mean 0,822 -0,267

p-probability: a review of the meta-pitting to pitting transition Chapter 4

85

4.3.2.4 Protection potential-PREN curve: experimental and theoretical values

comparison.

Protection potential values obtained from potentiodynamic tests are checked with Markov

model curves. Low PREN stainless steels experimental values show a good agreement

with the reviewed Markov model, as shown in Plot 4.11. For the p-probability curves

comparison will be, then, considered only AISI 304 and 430 stainless steels.

Plot 4.11- Eprot-PREN trend: theoretical and experimental comparison.

4.4 p-PROBABILITY CURVE:

EXPERIMENTAL AND THEORETICAL VALUES COMPARISON

On the following plots, p-probability curves are calculated using experimental results and

are compared with theoretical values. The reviewed Markov model p-probability curve is

obtained using in Eq. 4.6 protection potential values obtained from Eq. 4.4; experimental

p-probability values are obtained entering experimental protection potential in Eq.4.6: as

p-probability: a review of the meta-pitting to pitting transition Chapter 4

86

shown in Plot 4.12 and 4.13, they are reasonable, mostly considering that accelerated tests

are conducted under controlled procedures and in controlled environment; accordingly,

they predict lower pitting probability than theoretical model. Furthermore, mean values of

Epitt and Eprot are reported on the graphs (red circles) and compared with the reviewed

Markov model curve; a good match is obtained: at potential equal to mean experimental

protection potential a perfect match is obtained for both AISI 430 and 304 (pitting does not

propagate and p is equal to zero); at pitting potential a better match is obtained for AISI

304 but the results must be observed keeping in mind that the final pitting probability is 1-

R of Eq. 2.15, which takes into account also the chlorides concentration of the solution.

Indeed, at 20 g/L (Table 4.1) and at potential equal to 0, 066 V SCE, the pitting probability

1-R for AISI 430, calculated with Matlab®, is 99%.

Plot 4.12- p-probability curve for AISI 430 stainless steel and experimental values.

p-probability: a review of the meta-pitting to pitting transition Chapter 4

87

Plot 4.13- p-probability curve for AISI 304 stainless steel and experimental values.

m-probability: a review of the meta-stable to meta-passive transition Chapter 5

88

Chapter 5

m-PROBABILITY:

A REVIEW OF THE META-STABLE TO META-PASSIVE

TRANSITION

5.1 INTRODUCTION

The transitional probability m is the probability that a stainless steel in a specific

environment moves from the initial state of metastability to the condition of metapassivity.

m-probability depends on the ratio between chlorides concentration in the environment

([Cl-]) and critical chlorides threshold of the stainless steel ([Cl

-]cr):

Eq. 5.1

km

8,2exp1

Eq. 5.2 crCl

Clk

Figure 5.1- k dependence of m-probability.

m-probability: a review of the meta-stable to meta-passive transition Chapter 5

89

Figure 5.1 shows the dependence of m-probability on k: if the solution chlorides

concentration is, for example, 10 times higher than the critical chlorides threshold, m tends

quickly to zero; if [Cl-] is, instead, equal or lower than [Cl

-]cr m-probability is between 0,90

and 1. The breakdown of the passive film is more likely to occur as the chloride

concentration of the solution approaches the critical chloride content. Equation 5.3 shows

the relationship between critical chloride threshold and metallurgical, environmental and

geometrical factors (section 2.4.2):

Eq. 5.3

Since the relation between critical chlorides threshold and PREN is widespread among

corrosion engineers, the attention has been focused on pH and temperature dependence.

Experiments have been designed to get the critical chlorides concentration at three

different pH (2, 7 and 12) and at two different temperatures (20 °C and 40 °C) in order to

subsequently check them with Markov model trends (Figure 5.2 and 5.3).

Figure 5.2- Critical chlorides threshold dependence of pH: theoretical curves predicted by

Markov model for different stainless steel at 20°C and kcr= 0.

crevice

crevice

cr k

k

TpHPRENCl 3,0

4

1120

20

5,3

7

9log

m-probability: a review of the meta-stable to meta-passive transition Chapter 5

90

Figure 5.3- Critical chlorides threshold dependence of temperature: theoretical curves

predicted by Markov model for different stainless steels at pH 7 and Kcr equal to zero.

5.2 LINEAR POLARIZATION RESISTANCE TEST

Corrosion initiation is always associated with an increase of current density with respect to

that of the passive state; Linear Polarization Resistance (LPR) monitoring is an effective

electrochemical method of measuring corrosion current by means of a potentiostat and a

three-electrode electrochemical cell, shown in Figure 5.4 and described in section 3.2.

Between the sample (working electrode) and the reference electrode is applied a potential

which is scanned at constant rate (0,166 mV/s) from -10 mV vs Ecorr to +10 mV vs Ecorr

and the circulating current is measured and normalized with respect to the surface area [7].

m-probability: a review of the meta-stable to meta-passive transition Chapter 5

91

Figure 5.4- Schematic representation of the electrochemical cell: CE is the counter

electrode (Ti-MMO), W the working electrode (stainless steel sample) and ER the

reference electrode (SSCsat).

At potential very close to Ecorr the slope of the potential-current curve,

i

E, is

approximately linear (Fig. 5.5) and has the units of resistance (Eq. 5.4)

Eq. 5.4 i

ELPR

[Ω] if (E-Ecorr) 0

The measured resistance is inversely related to the corrosion current:

Eq. 5.5 LRP

B

E3,2

ii

ca

ca

corr

Where βa and βc are anodic and cathodic Tafel slopes and B is the Stern-Geary coefficient.

Representing the polarization curve as a linear potential-current density plot, the

polarization resistance LPR is determined as the tangent of the curve at i=0.

m-probability: a review of the meta-stable to meta-passive transition Chapter 5

92

Figure 5.5 Measurement of icorr by linear polarization [2].

Polarization resistance and corrosion potential monitoring provides information about

pitting corrosion. A simultaneously drop of LPR and potential suggests passive layer

breakdown and increase of corrosion rate. This is explained considering the inverse

proportionality between polarization resistance and current density (Eq 5.5); furthermore,

Figure 5.6 shows that a lower corrosion potential means an active behavior of stainless

steel. If the system works at point A, the material is passive and characterized by noble

potential and low corrosion current density; when the passive film breakdown occurs,

stainless steel anodic curve is like that of an active material (Fig. 5.6, dashed line) and the

working point of the system becomes B: the potential drop from A to B is matched with an

increase of current density.

m-probability: a review of the meta-stable to meta-passive transition Chapter 5

93

Figure 5.6- Schematic illustration of the electrochemical concept of potential decrease.

5.3 EFFECT OF pH ON CRITICAL CHLORIDES THRESHOLD

5.3.1 Aim of the test

In order to get the pH-critical chlorides concentration trend, the following experiment has

been designed. Three tanks, containing NaCl solution, were set up: one at pH 2, one at pH

7 and one at pH 12. In each tank were immersed five samples of AISI 304 stainless steel,

whose potential and LPR variation in time was monitored. Every 48 hours the chlorides

concentration was increased until a simultaneous decrease of potential and LPR occurs: the

chlorides content corresponding to this simultaneous variation is the critical chlorides

threshold.

5.3.2 Experimental set-up

Fifteen AISI 304 stainless steel samples (size 1 x 1 cm) were cut from sheets of dimensions

18 x 27 x 0.1 cm. They were electrically connected to an insulated electrical cable by spot

welding of the back surface. The sample surface, which will be exposed to the solution,

was then positioned to the bottom of a lubricated teflon couvette and the back surface was

m-probability: a review of the meta-stable to meta-passive transition Chapter 5

94

covered with an epoxy resin (Fig. 5.7). After 24 hours, the sample was extracted from the

sample-holder and the exposed surface finished with abrasive papers. The sample is shown

in Figure 5.8.

Figure 5.7- Sample in the teflon couvette. Figure 5.8- Finished sample.

The test solutions were prepared with 2 L of distilled water and different concentration of

sodium chlorides, depending on the pH. The initial chlorides concentration were: 50 mg/L

at pH 7, 10 mg/L at pH 2 and 300 mg/L at pH 12. Acid solution was obtained adding 0,981

g of H2SO4; alkaline solution adding 8 g of NaOH.

For each becker a cover with five holes for the samples and two holes for the reference and

counter electrodes was prepared. Holes allow the passage of electric cables (Fig. 5.9). Five

sample were immersed in each becker and a shunt was mounted at the end of each cable

(Fig.5.10). Every 48 hours potential and LPR were monitored (Fig. 5.11) and chlorides

concentration was increased by the addition of sodium chlorides to the solution.

m-probability: a review of the meta-stable to meta-passive transition Chapter 5

95

Fig. 5.9- Cables passage into cover holes and

sample immersion.

Fig. 5.10- Becker cover.

Fig. 5.11- Electrical connection and monitoring.

m-probability: a review of the meta-stable to meta-passive transition Chapter 5

96

5.3.3 Results

5.3.3.1 pH= 2

Plot 5.1 and 5.2 show potential and LPR variation with time. Sample 1 and sample 5 are

affected by a potential drop which, however, is not matched with a LPR drop; anyway, the

determination of the critical chlorides content (corresponding to the day when a sensible

decrease of potential and LPR occurs) is possible and reported in Table 5.1. The variation

in the electrochemical behavior of sample 2, 3, and 4 is difficult to recognize: potential and

polarization resistance trend is quite constant in time and corrosion current density is, since

the first day after immersion, of the order of 10 mA/m2; since, at pH 2, AISI 304 stainless

steel may be subject of a corrosion attack uniformly distributed over the entire surface (see

section 2.3.1); the idea, which agrees with experimental results, is that for samples 2, 3 and

4 general corrosion occurred.

Table 5.1- Critical chlorides threshold at pH 2.

pH Sample [Cl]cr (mg/L) Mean value (mg/L) Minimum value (mg/L)

2

1 4000

2750 1500

2 -

3 -

4 -

5 1500

m-probability: a review of the meta-stable to meta-passive transition Chapter 5

97

Plot 5.1- Potential- time trend at pH 2.

Plot 5.2- LPR-time trend at pH 2.

m-probability: a review of the meta-stable to meta-passive transition Chapter 5

98

5.3.3.2 pH= 7

Plot 5.3 and 5.4 show potential and LPR variation with time for the five samples at pH 7

and Table 5.2 reports critical chlorides thresholds and their mean value. Also in this case,

trends are difficult to interpret; instability phenomena, like metastable pits, may be

occurred: this is shown by the “up and down” trend of both potential and LPR. Critical

chlorides concentration is chosen to be that corresponding to potential and resistance

stabilization to the lower values: potential decreases from about 100 mV SSC (passive

condition) to -200 mV SSC (active condition), while LPR decreases from values of the

order of 107 Ω, which corresponds to passive currents lower than 1 mA/m

2, to values of the

order of 105 Ω, which corresponds to corrosion current higher than 2 mA/m

2.

Sample 5 has an anomalous behavior: potential of the order of -150 mV SSC, which

remains stable in time, and LPR which decreases progressively from initial values of the

order of 105 to values of the order of 10

4; this can be explained assuming a less stable

passive film, maybe deriving by some inaccuracy during sample preparation.

Table 5.2- Critical chlorides threshold at pH 7.

pH Sample [Cl]cr (mg/L) Mean value Minimum value

7

1 30000

17500 10000

2 15000

3 15000

4 10000

5 -

m-probability: a review of the meta-stable to meta-passive transition Chapter 5

99

Plot 5.3- Potential-time trend at pH 7.

Plot 5.4- LPR-time trend at pH 7.

m-probability: a review of the meta-stable to meta-passive transition Chapter 5

100

5.3.3.3 pH= 12

Plot 5.5- Potential-time trend at pH 12.

Plot 5.6- LPR-time trend at pH 12.

m-probability: a review of the meta-stable to meta-passive transition Chapter 5

101

Plots 5.5 and 5.6 show potential and LPR variation with time for the five samples at pH 12.

Also in this case, the “up and down” trend of both potential and LPR suggests that

metastable pits may be started; anyway, the critical chlorides threshold cannot be identified

because there is not an evident and permanent variation in the electrochemical behavior of

the samples.

5.3.4 Discussion

The first consideration that must be done is about the absolute value of the critical

chlorides threshold. It’s evident that, for example, a critical chlorides threshold of 20.000

ppm at pH 7 is not reasonable: corrosion experience suggests that AISI 304 stainless steel

critical chloride content at neutral pH, room temperature and stagnant condition is about

50-100 ppm. As already discussed in Chapter 3, it’s important to take into account the

limitation of laboratory experiments in order to interpret carefully the results of these tests.

Laboratory experiments are carried out under controlled condition during which there isn’t

any temperature, pH or chlorides concentration variation; sample surface is small (1 cm2)

compared to exposed surface in real system components and then the probability to find

pitting initiation sites (surface defects) decreases. Another critical point is experiments

duration: initiation time for pits formation is a stochastic parameter very difficult to

predict; laboratory experiments are accelerated test for practical reasons and, even if

widespread accepted and used, may lead to misleading results. It follows that two days

maybe are not sufficient to initiate corrosion at a fixed chlorides concentration.

For comparison purposes, the experimental pH-critical chlorides threshold trend and the

Markov one (for PREN 18 stainless steel, at 20°C, and kcr equal to zero) are reported on

the same graph (Plot 5.7): as discussed, absolute values of chlorides threshold are not

reliable but the linear trend is respected; the pH= 12 critical chlorides threshold reported on

Plot 5.7 is the chlorides concentration of the last day of the experimental tests (200.000

mg/L).

As the slope of the old Markov model and experimental straight lines is quite different, the

idea is to change the A constant of Eq. 5.4, which for Markov model is equal to 3,5:

Eq. 5.4

A

pHCl cr

7log

m-probability: a review of the meta-stable to meta-passive transition Chapter 5

102

The experimental curve is then shifted toward lower values: the boundary condition is

chlorides threshold at pH 7 equal to zero and the experimental straight line is then fixed at

the point B. While old Markov model trend was that each 3,5 pH unit the critical threshold

increased of one order of magnitude, the experimental trend shows that each 5 pH unit [Cl-

]cr increases of about one order of magnitude (Eq. 5.5); then, the new A constant is equal to

5:

Eq. 5.5

Plot 5.7- Experimental data elaboration: reviewed pH- chlorides threshold trend.

5

7log

pHCl cr

m-probability: a review of the meta-stable to meta-passive transition Chapter 5

103

5.4 EFFECT OF TEMPERATURE ON CRITICAL CHLORIDES THRESHOLD

5.4.1 Aim of the test

In order to get the temperature-critical chlorides threshold trend, potential and LPR

monitoring has been carried out for five samples at 40°C and neutral pH. The 20°C results

are considered those at pH 7 of section 5.3.3.2.

5.4.2 Experimental set up

The test material is AISI 304 stainless steel and five samples were prepared as described in

section 5.3.2. The test solution was prepared with 1,6 L of distilled water and an initial

chlorides concentration of 100 mg/L. The cover with five holes for the sample electric

cables and two holes for the reference and counter electrodes was prepared. Five sample

were immersed in the glass becker and a shunt was mounted at the end of each cable, as

already shown in Fig. 5.10.

In order to raise solution temperature to 40°C and maintain it during the experiment

duration, an heating plate was used which had been connected with a Vertex, a digital

thermoregulator for direct temperature control of the liquid (Fig. 5.12). Every 48 hours

potential and LPR were monitored and chlorides concentration increased by the addition of

sodium chlorides to the solution.

m-probability: a review of the meta-stable to meta-passive transition Chapter 5

104

Fig. 5.12- 40° C test set up and cables for potential and LPR monitoring.

5.4.3 Results

Plots 5.8 and 5.9 show potential and LPR variation with time and in Table 5.3 are reported

the critical chloride thresholds and their mean value. Also in this case the trends are

difficult to interpret because there is not always an evident drop in potential and

polarization resistance; anyway, sample 1 shows a 250 mV and samples 4 and 5 a 50 mV

of potential drop matched with LPR decrease, which from values of the order of 106 Ω

decreases to values of the order of 104-10

5 Ω; sample 2 and 3 show, instead, a potential

stabilization in time to high potential values.

Table 5.3- Critical chlorides threshold at 40°C.

Temperature Sample [Cl]cr (mg/L) Mean value Minimum value

40

1 15000

7000 2000

2 -

3 -

4 2000

5 5000

m-probability: a review of the meta-stable to meta-passive transition Chapter 5

105

Plot 5.8- Potential-time trend at 40°C.

Plot 5.9- LPR-time trend at 40°C.

m-probability: a review of the meta-stable to meta-passive transition Chapter 5

106

5.4.4 Discussion

The considerations done about experimental corrosion tests limitation (section 5.3.4) are

relevant also in this case and the data elaboration which follows is methodologically

similar to that realized for the pH trend. The experimental and the Markov model curves

are compared in Plot 5.10: the critical chlorides threshold of 100 ppm for PREN 18

stainless steel at 20°C and pH 7 is chosen again as boundary condition; then, the curve is

shifted to lower values and fixed at point B; the aim is to evaluate the slope variation and

change the A constant of Eq. 5.6, which, for Markov model, is equal to 20:

Eq. 5.6

Plot 5.10- Experimental data elaboration: reviewed temperature- critical chlorides

threshold trend.

A

TCl cr

20log

m-probability: a review of the meta-stable to meta-passive transition Chapter 5

107

Experimental data show that critical chlorides threshold decreases one order of magnitude

each 40°C increase (Eq. 5.7), instead each 20°C as predicted by the old Markov model; A

constant is then equal to 40, as shown in Eq. 5.7.

Eq. 5.7

5.5 CALCULATION OF m-PROBABILITY

As already discussed, the PREN dependence of critical chlorides threshold has not been

modified because widespread among corrosion engineers and the crevice parameter has not

been studied yet. The m-probability equation becomes:

Eq. 5.8

Table 5.5 shows how m-probability changes varying pH and the reviewed probability is

compared with the old one. Values are obtained through Matlab® elaboration.

Table 5.5- pH dependence of old Markov and new Markov model m-probability.

PREN Temperature (°C) Chlorides (mg/L) pH m-probability

old Markov

m-probability

new Markov

18 20 1000

2 0,0104 0,0276

7 0,2442 0,2442

12 0,9995 0,9392

As expected, m-probability (meta-stable to meta-passive transition) increases as pH

increases because alkaline condition favors repassivation. Reviewed m-probability at pH 2

is higher than that of Markov model: laboratory tests results show an high resistance to

pitting for samples at pH 2. At neutral pH (and 20°C) m-probability does not change

respect to “old” Markov model because of the choice of the boundary condition for data

40

20log

TCl cr

crevice

crevice

cr k

k

TpHPRENCl 3,0

4

1140

20

5

7

9log

m-probability: a review of the meta-stable to meta-passive transition Chapter 5

108

elaboration (section 5.3.4). At alkaline pH reviewed m-probability results lower because of

the change in the slope of the pH-critical chlorides threshold straight line (Plot 5.7).

The effect of temperature on m-probability is shown in Table 5.6: m-probability decreases

as the temperature increases, as expected. The reviewed probabilities are higher than the

“old” because experimental tests show an higher pitting resistance of the material. This

trend changes for temperature lower than 20°C because of the slope of the temperature-

critical threshold straight line.

Table 5.6- Temperature dependence of old Markov and new Markov model m-probability.

PREN Temperature (°C) Chlorides

(mg/L) pH

m-probability

old Markov

m-probability

new Markov

18

20

1000 6

0,1350 0,1619

40 0,0144 0,0543

60 0,0014 0,0028

Table 5.7- Chlorides concentration dependence of old and new Markov model m-probability.

PREN Temperature (°C) Chlorides

(mg/L) pH

m-probability

old Markov

m-probability

new Markov

18

40

100

6

0,1350 0,4280

1000 0,0144 0,0543

20000 0,00072 0,0028

Table 5.7 shows a decrease of meta-stable to meta-passive transition probability as

chlorides concentration increases because higher chlorides lead to less strong passive film.

The reviewed probabilities, as expected, are higher.

Plot 5.11 shows a compare of old Markov and new Markov model m-probability curve for

three different stainless steels at pH 6, 25°C and kcr equal to zero. It shows an higher

metastable to metapassive transition probability: for example, for PREN 18 stainless steel

at 100 ppm chlorides the old Markov m-probability was 55% while the new one is 73%; a

PREN 40 duplex stainless steel shows an m-probability equal to one until about 8000 ppm

chlorides; it decreases to 70% at 25000 ppm for the old model and 30000 ppm for the new

one; one can also observe that increasing the PREN, the difference between the two model

decreases.

m-probability: a review of the meta-stable to meta-passive transition Chapter 5

109

Plot 5.11- Compare between old and new Markov m-probability dependence for different

stainless steel at pH 6, 25°C and kcr equal to zero on chlorides concentration.

In order to complete the m-probability review, crevice effect must be studied; furthermore,

some consideration about Eq. 5.1 should be done. Considering what already examined and

modified, in the following and last chapter a compare between reviewed, old Markov and

experimental pitting probabilities (1-R) is shown.

Conclusion Chapter 6

110

Chapter 6

CONCLUSION

In the industrial field, localized corrosion of stainless steels, as pitting and crevice, is a

critical issue. Since, once pits initiate, their propagation is fast and generally unstoppable,

the major effort of corrosion engineers is focused on the prediction of the initiation time.

Pitting corrosion and its initiation are intrinsically stochastic phenomena and for their

description a probabilistic approach is mandatory. In this work is proposed a Markov

chain’s mathematical model which assumes that pitting retains no memory of its past

history and is characterized by two absorbing states (pitting and repassivation) and three

transitional states (metastable, metapassive, metapitting), as shown in Fig. 6.1; the model

takes into account metallurgical and environmental factors, as material composition

(PREN), chlorides concentration, pH, temperature, fluidodynamic condition and oxidant

power of the system, with the aim to calculate the corrosion probability of stainless steels

in environments. By means of literature data elaboration and laboratory tests, the

equations, which relates the aforementioned parameters with the transitional probabilities

(in particular m and p), initially empirical expressions based on engineering knowledge of

corrosion behavior of stainless steels, are revised and partly modified. The new equations

are reported in the following.

Fig. 6.1- Five-step Markov model.

Conclusion Chapter 6

111

6.1 p-probability: new Markov model equation

The probability to move from the metapitting state to the pitting absorbing state depends

on the difference between the potential of the material in a specific environment and the

protection potential (Eq. 6.1). If the system is on cathodic protection ( protEE ) p-

probability is equal to zero because corrosion is not thermodynamically possible.

Eq. 6.1

3

protEE2

3exp1p

0p

prot

prot

EE

EE

The protection potential is assumed to be linear dependent on PREN (Eq. 6.2) but

independent on the chlorides concentration, which plays an important role in defining,

instead, m-probability.

Eq. 6.2 40

PREN760,0Eprot V SCE

6.2 m-probability: new Markov model equation

The probability that the system evolves from the metastable condition to the metapassive

state depends on the ratio k between the solution chlorides concentration [Cl-] and the

critical chlorides threshold [Cl-]cr (Eq. 6.3).

Eq. 6.3

km

8,2exp1 , where

Eq. 6.4 crCl

Clk

Conclusion Chapter 6

112

Eq. 6.5 shows the relationship between critical chloride content and metallurgical,

environmental and geometrical factors; in this work, the elaboration was focused on

temperature and pH dependence.

Eq. 6.5

6.3 r-probability: the existing Markov model equation

The probability r is the probability that a stainless steel in a specific environment moves

from the metapassive condition to the absorbing state of passivity. It depends on the

fluidodynamic condition of the system (fluid velocity) and on stainless steel PREN; these

dependence have not been study and Equations 6.6 and 6.7 are the originals:

Eq. 6.6 4

min v2,0expr11r

Eq. 6.7

2,3

min50

PRENr

6.4 Final consideration and future perspective

In Tables 6.1, 6.2 and 6.3 the experimental corrosion probabilities for AISI 430, 304 and

470LI stainless steels are compared with the old Markov model pitting probabilities and

with those reviewed (calculated by means of Matlab®): especially for the less aggressive

conditions, the gap between experimental and Markov model corrosion probabilities is

decreased. For example for AISI 430 at 20°C and pH 7 the corrosion probability decreases

from 42% to 14%; at polarization potential + 0,300 mV vs Ecorr and 1000 mg/L Cl- it

remains unchanged for low PREN stainless steels and decreases, instead, from 96% to 28%

for PREN 24 stainless steel.

crevice

crevice

cr k

k

TpHPRENCl 3,0

4

1140

20

5

7

9log

Conclusion Chapter 6

113

Table 6.1- AISI 430 (PREN 17) experimental corrosion probability and Markov probabilities.

T (°C) pH Cl (mg/L) E (V SCE) Pc

EXP

1-R

Old Markov model

1-R

Reviewed Markov model

20 7

100

-0,014

0% 42% 14%

300 0% 84% 55%

1000 0% 96% 84%

100

-0,156

10% 64% 57%

300 5% 93% 91%

1000 60% 98% 98%

40 7

100

-0,014

0% 97% 77%

300 0% 99% 93%

1000 0% 100% 98%

100

0,281

95% 99% 95%

300 100% 100% 99%

1000 100% 100% 100%

Table 6.2- AISI 304 (PREN 18) experimental corrosion probability and Markov probabilities.

T (°C) pH Cl (mg/L) E (V SCE) Pc

EXP

1-R

Old Markov model

1-R

Reviewed Markov model

20 7

100

0,056

0% 34% 21%

300 0% 84% 72%

1000 0% 96% 93%

100

0,166

15% 42% 34%

300 0% 88% 84%

1000 10% 97% 96%

40 7

100

-0,014

0% 95% 61%

300 0% 98% 97%

1000 0% 100% 96%

100

0,256

15% 98% 89%

300 0% 99% 97%

1000 25% 100% 99%

Conclusion Chapter 6

114

Table 6.3- 470LI (PREN 24) experimental corrosion probability and Markov probabilities.

T (°C) pH Cl (mg/L) E (V

SCE)

Pc

EXP

1-R

Old Markov model

1-R

Reviewed Markov model

20 7

100

-0,094

0% 0% 0%

300 0% 1% 0%

1000 0% 24% 2%

100

0,156

5% 0% 0%

300 5% 4% 1%

1000 15% 96% 28%

40 7

100

0,006

0% 38% 3%

300 0% 75% 52%

1000 0% 92% 24%

100

0,246

5% 60% 3%

300 0% 88% 42%

1000 10% 97% 81%

More work should be made to improve this five-steps Markov model, as laboratory tests, in

order to obtain reliable values of protection potential for high PREN stainless steels (as

potentiodynamic tests in deareated solution and potentiostatic scratch tests), and field tests,

in order to compare “in field” corrosion probabilities to that predicted by Markov model.

Furthermore, the crevice dependence of the critical chlorides threshold (Eq. 6.5) and r-

probability dependence on fluidodynamic condition of the system (Eq. 6.6 and 6.7) must

be studied.

Literature data collection APPENDIX A

115

APPENDIX A: Literature data collection.

PREN Cl (mg/L) Epitt ( V SCE) Reference PREN Cl (mg/L) Epitt ( V SCE) Reference

12 21000 -0,060 [2] 21 17500 0,430 [1]

13 21000 -0,200 [11] 21 26000 0,320 [1]

14 21000 -0,300 [11] 21 35000 0,202 [1]

16 21000 0,100 [11] 21 35000 0,195 [1]

16 21000 -0,100 [11] 21 35000 0,170 [1]

17 21000 0,025 [1] 22 21000 0,120 [11]

17 21000 -0,080 [1] 22 21000 0,150 [11]

17 17000 0,090 [1] 22 35000 0,030 [11]

17 26000 -0,010 [1] 22 21000 0,490 [36]

17 35000 -0,050 [1] 22 18000 0,290 [1]

17 18000 -0,050 [1] 22 18000 0,230 [1]

17 18000 -0,010 [1] 23 30000 0,256 [37]

17 30000 -0,034 [37] 23 21000 0,000 [11]

18 21000 0,110 [35] 24 35000 0,297 [1]

18 30000 -0,024 [37] 24 35000 0,224 [1]

18 21000 -0,045 [11] 25 19000 0,388 [36]

18 21000 -0,080 [11] 25 21000 0,410 [35]

18 21000 -0,070 [11] 25 22000 0,365 [36]

18 35000 0,200 [1] 25 25000 0,332 [36]

18 35000 0,500 [1] 25 6000 0,335 [11]

18 21000 -0,060 [11] 25 20000 0,335 [11]

18 21000 0,000 [11] 25 90000 0,245 [11]

18 35000 -0,200 [11] 26 30000 0,116 [37]

18 21000 0,280 [35] 26 21000 0,530 [35]

18 21000 0,290 [1] 26 21000 0,140 [11]

18 18000 0,030 [1] 29 35000 0,423 [1]

18 18000 0,080 [1] 29 35000 0,413 [1]

18 30000 0,056 [37] 31 21000 0,420 [11]

18 21000 0,280 [35] 33 30000 0,956 [37]

18 35000 0,090 [1] 34 35000 0,637 [1]

18 35000 0,095 [1] 34 35000 0,680 [1]

19 17500 0,300 [1] 44 19000 1,075 [36]

19 26000 0,150 [1] 44 22000 1,025 [36]

19 35000 -0,050 [1] 44 25000 1,002 [36]

19 21000 -0,220 [1] 45 19000 1,182 [36]

20 17500 0,190 [1] 45 22000 1,125 [36]

20 26000 0,020 [1] 45 25000 1,108 [36]

20 35000 -0,070 [1] 46 19000 1,221 [36]

Literature data collection APPENDIX A

116

PREN Cl (mg/L) Epitt ( V SCE) Reference

46 22000 1,158 [36]

46 25000 1,139 [36]

52 19000 1,249 [36]

52 22000 1,182 [36]

52 25000 1,174 [36]

Density and cumulative distribution of the collected pitting potential APPENDIX B

117

APPENDIX B: Density and cumulative distribution of the collected pitting potential.

Mean Epitt (V SCE) 0,255 E (V SCE) Density Cumulative

St. dev. (V SCE) 0,232 0,125 1,471 0,287

0,150 1,553 0,325

E (V SCE) Density Cumulative 0,175 1,622 0,365

-0,700 0,000 0,000 0,200 1,674 0,406

-0,675 0,001 0,000 0,225 1,707 0,448

-0,650 0,001 0,000 0,250 1,721 0,491

-0,625 0,001 0,000 0,275 1,715 0,534

-0,600 0,002 0,000 0,300 1,690 0,577

-0,575 0,003 0,000 0,325 1,645 0,618

-0,550 0,004 0,000 0,350 1,583 0,659

-0,525 0,006 0,000 0,375 1,506 0,698

-0,500 0,009 0,001 0,400 1,416 0,734

-0,475 0,012 0,001 0,425 1,316 0,768

-0,450 0,017 0,001 0,450 1,209 0,800

-0,425 0,023 0,002 0,475 1,098 0,829

-0,400 0,032 0,002 0,500 0,985 0,855

-0,375 0,043 0,003 0,525 0,874 0,878

-0,350 0,057 0,005 0,550 0,766 0,898

-0,325 0,075 0,006 0,575 0,664 0,916

-0,300 0,098 0,008 0,600 0,569 0,932

-0,275 0,126 0,011 0,625 0,482 0,945

-0,250 0,160 0,015 0,650 0,403 0,956

-0,225 0,201 0,019 0,675 0,333 0,965

-0,200 0,250 0,025 0,700 0,273 0,973

-0,175 0,307 0,032 0,725 0,220 0,979

-0,150 0,373 0,040 0,750 0,176 0,984

-0,125 0,448 0,050 0,775 0,139 0,988

-0,100 0,532 0,063 0,800 0,108 0,991

-0,075 0,624 0,077 0,825 0,084 0,993

-0,050 0,723 0,094 0,850 0,064 0,995

-0,025 0,829 0,113 0,875 0,048 0,996

0,000 0,939 0,135 0,900 0,036 0,997

0,025 1,051 0,160 0,925 0,026 0,998

0,050 1,164 0,188 0,950 0,019 0,999

0,075 1,273 0,218 0,975 0,014 0,999

0,100 1,376 0,252 1,000 0,010 0,999

Density and cumulative distribution of the collected pitting potential APPENDIX B

118

Pitting potential cumulative distribution. Cumulative function used as model curve.

Eprot -0,298 V SCE

P% Epitt P E (V SCE) E-Eprot

5% -0,126 0,05 -0,126 0,172

10% -0,042 0,1 -0,042 0,256

15% 0,015 0,15 0,015 0,312

20% 0,060 0,2 0,060 0,358

25% 0,099 0,25 0,099 0,396

30% 0,134 0,3 0,134 0,431

35% 0,166 0,35 0,166 0,463

40% 0,196 0,4 0,196 0,494

45% 0,226 0,45 0,226 0,524

50% 0,255 0,5 0,255 0,553

55% 0,284 0,55 0,284 0,582

60% 0,314 0,6 0,314 0,611

65% 0,344 0,65 0,344 0,642

70% 0,377 0,7 0,377 0,674

75% 0,411 0,75 0,411 0,709

80% 0,450 0,8 0,450 0,748

85% 0,495 0,85 0,495 0,793

90% 0,552 0,9 0,552 0,850

95% 0,636 0,95 0,636 0,934

99% 0,794 0,99 0,794 1,092

REFERENCES

119

REFERENCES

[1] A. J. Sedriks, Corrosion of stainless steels, Wiley, 1979, pp. 282.

[2] Austenitic stainless steels, ASM International, Material Park, Ohio, USA.

[3] R. W. Revie, Uhlig’s corrosion handbook, 2nd

Ed., Wiley, 2000, pp. 1302.

[4] P. Pedeferri, Corrosione e protezione dei materiali metallici, Polipress, 2007, pp. 408.

[5] M. Pourbaix, Atlas of electrochemical equilibria in aqueous solutions, 2nd

Ed.,

Houston: National association of corrosion engineers, 1974, pp. 644.

[6] G.S. Frankel, Localized corrosion of metals: a review of the rate controlling factors in

initiation and growth, Electrochemical Society Proceedings, Vol. 99-42, pp. 445-475.

[7] J.R. Scully, Corrosion tests and standards manual, 2nd

Ed., R. Baboian Editor, 2005,

pp. 882.

[8] P. Pedeferri, Metodi di prevenzione e protezione, Corso di corrosione e protezione dei

materiali 2004-2005, Politecnico di Milano.

[9] V. Boneschi, M. Boniardi, Gli acciai inox e la resistenza alla corrosione, Lamiera,

2008, pp. 124-131.

[10] W. Nicodemi, Metallurgia, Principi generali, 2nd Ed., Zanichelli, 2007, pp. 352.

[11] L.L Sheir, R.A. Jarman and G.T Burstein, Corrosion Metal/Environment reactions, 3rd

Ed.,Vol.1, Butterworth Heinemann, 2000, pp. 3:35-3:77.

[12] G. Salvago, G. Fumagalli, Valutazione degli effetti delle condizioni metallurgiche e della

finitura superficiali sulla probabilità di attacco localizzato di acciai inossidabili, Atti,

Giornate nazionali sulla corrosione e protezione, 24-25 Maggio 1994, pp. 225-232.

[13] L. Magagnin, G. Salvago, Statistical evaluation of localized corrosion for stainless

steels ranking, Corrosion Reviews, Vol. 19, Nos 3-4, 2001, pp. 347-366.

REFERENCES

120

[14] A. Pardo, E. Otero, M.C. Merino, M.D. López, M.V. Utrilla, F. Moreno, Influence of

pH and chloride concentration on the pitting and crevice corrosion behavior of high-alloy

stainless steels, Corrosion engineering section, 2000, pp. 411-418.

[15] H. M. Ezuber, Metallurgical and environmental factors affecting the pitting behavior

of UNS S32205 duplex stainless steel in chloride solutions, Materials and Corrosion No. 2,

2012, pp. 111-118..

[16] S. Ravasio, Modello statistico a catena di Markov per la previsione dell’innesco del

pitting su acciai inossidabili, Tesi di laurea di primo livello, Politecnico di Milano, 2008,

pp. 51.

[17] L. Lazzari, M. Ormellese, S. Ravasio, Modello a matrici di Markov per la previsione

dell’innesco del pitting di acciai inossidabili, Politecnico di Milano.

[18] T. Shibata, Statistical and stochastic approaches to localized corrosion, W.R.

Whitney Award Lecture, 1996, pp. 813-829.

[19] R. Fratesi, Statistical estimate of the pitting potential of AISI 319L stainless steel in

3.5% NaCl measured by means of two electrochemical methods, Corrosion NACE, Vol.

41, 1985, pp. 114-117.

[20] G. Salvago, G. Fumagalli, The distribution of the breakdown potential of stainless

steels: effects of test repetition, specimen exposure surfaces and threshold current,

Corrosion science, Vol. 37, No 8, 1995, 1303-1311.

[21] J. W. Provan, E. S. Rodrguez III, Part I: Development of a Markov description of

pitting corrosion, Corrosion, 1989, pp. 177-192.

[22] ASTM G46, Standard guide for examination and evaluation of pitting corrosion,

Reapproved 2005.

REFERENCES

121

[23] P. Citti, G. Arcidiacono, G. Campatelli, Fondamenti di affidabilità, McGraw-Hill,

2003, pp. 192.

[24] F. Caleyo, J.C. Velazquez, A. Valor, J.M. Hallen, Markov chain modelling of pitting

corrosion in underground pipelines, Corrosion Science, Vol. 51, 2009, pp. 2197-2207.

[25] E. S. Rodriguez III, On a new Markov model for the pitting corrosion process and its

application to reliability, Work of thesis, McGill university, Montreal, 1986, pp. 273.

[26] C. M. Grinstead, J.L. Snell, Introduction to probability, 2nd

Ed., American

mathematical society, 2006, pp. 405-470.

[27] H. P. Hong, Application of the stochastic process to pitting corrosion, Corrosion,

1999, pp. 10-16.

[28] F. Caleyo, J.C. Velazquez, A. Valor, J.M. Hallen, Markov chain modelling of pitting

corrosion in underground pipelines, Corrosion Science, Vol. 51, 2009, pp. 2197-2207.

[29] A. Valor, F. Caleyo, L. Alfonso, D. Rivas, J.M. Hallen, Stochastic modelling of

pitting corrosion: a new model for initiation and growth of multiple corrosion pits,

Corrosion Science, Vol. 49, 2007, pp. 559-579.

[30] F. Bolzoni, P. Fassina, G. Fumagalli, L. Lazzari, E. Mazzola, Application of

probabilistic models to localized corrosion study, Metallurgia Italiana 98, 2006, pp. 9-15.

[31] G. Contreras, P. Fassina, G. Fumagalli, S. Goidanich, L. Lazzari, E. Mazzola, A study

on metastability phenomena of passive films for corrosion resistant alloys, Electrochemical

acta, 2007, pp. 1-22.

[32] C. Alonso, M. Castellote, C. Andrade, Chloride threshold dependence of pitting

potential of reinforcements, Electrochimica Acta, Vol. 47, 2002, pp. 3469-3481.

[33] T. Shibata, Corrosion probability and statistical evaluation of corrosion data,

Uhlig’s corrosion handbook, 2nd

Ed., Wiley, 2000, pp. 367-391.

REFERENCES

122

[34] ASTM G31, Standard practice for laboratory immersion corrosion testing of metals,

2012.

[35] L. Felloni, R. Fratesi, O. Ruggeri, G. Sambogna, Pitting ad crevice corrosion

potentials of sola1 panel stainless steels in seawater and 0.6M NaCl, Corrosion NACE,

Vol. 41, 1985, pp. 169-177.

[36] G. Latha, S. Rajeswari, Pitting and crevice corrosion behavior of superaustenitic

stainless steel in sea water cooling system, Corrosion Reviews, Vol.18, No.6, 2000, pp.

429-456.

[37] R.W. Staehle, B.F. Brown, Localized corrosion, NACE 1, 1974, pp. 749.

[38] ASTM G61, Standard test method for conducting cyclic potentiodynamic polarization

measurements for localized corrosion susceptibility of iron-, nickel-, or cobalt-based

alloys, Reapproved 2009.

Recommended